Spark Plasma Sintering of Si N-Based Ceramics - DiVA …Spark Plasma Sintering of Si3N4-Based...
Embed Size (px)
Transcript of Spark Plasma Sintering of Si N-Based Ceramics - DiVA …Spark Plasma Sintering of Si3N4-Based...
Spark Plasma Sintering of Si3N4-Based Ceramics -Sintering mechanism-Tailoring microstructure-Evaluating properties-
HONG PENG 彭 红
Department of Inorganic Chemistry Stockholm University
Doctoral Dissertation 2004 Department of Inorganic Chemistry Stockholm University S-10691 Stockholm Sweden Faculty opponent:
Prof Michael J. Hoffmann
Institute for Ceramics in Mechanical Engineering University of Karlsruhe, Haid-und-Neu-Str. 7 D-76131 Karlsruhe Germany Evaluation committee:
Prof Sven Lidin, Department of Inorganic Chemistry, Stockholm University Prof Richard Warren, IPF Materialvetenskap, Malmö högskola, 205 06 Malmö Dr Magnus Ekelund, Sandvik Coromant AB Doc Ulrich Häussermann, Department of Structural Chemistry, Stockholm University
© Hong Peng ISBN 91-7265-834-7 Intellecta DocuSys, Stockholm 2004
In the memory of my father
To my mother 献给我的妈妈
Work while you work;
Play while you play;
This is the way;
To be cheerful and gay.
── A. D. Stoddart
ABSTRACT Spark Plasma Sintering (SPS) is a promising rapid consolidation technique that allows a better understanding and manipulating of sintering kinetics and therefore makes it possible to obtain Si3N4-based ceramics with tailored microstructures, consisting of grains with either equiaxed or elongated morphology. The presence of an extra liquid phase is necessary for forming tough interlocking microstructures in Yb/Y-stabilised α-sialon by HP. The liquid is introduced by a new method, namely by increasing the O/N ratio in the general formula RExSi12-
(3x+n)Al3x+nOnN16-n while keeping the cation ratios of RE, Si and Al constant. Monophasic α-sialon ceramics with tailored microstructures, consisting of either fine equiaxed or elongated grains, have been obtained by using SPS, whether or not such an extra liquid phase is involved. The three processes, namely densification, phase transformation and grain growth, which usually occur simultaneously during conventional HP consolidation of Si3N4-based ceramics, have been precisely followed and separately investigated in the SPS process. The enhanced densification is attributed to the non-equilibrium nature of the liquid phase formed during heating. The dominating mechanism during densification is the enhanced grain boundary sliding accompanied by diffusion- and/or reaction-controlled processes. The rapid grain growth is ascribed to a dynamic ripening mechanism based on the formation of a liquid phase that is grossly out of equilibrium, which in turn generates an extra chemical driving force for mass transfer. Monophasic α-sialon ceramics with interlocking microstructures exhibit improved damage tolerance. Y/Yb- stabilised monophasic α-sialon ceramics containing approximately 3 vol% liquid with refined interlocking microstructures have excellent thermal-shock resistance, comparable to the best β-sialon ceramics with 20 vol% additional liquid phase prepared by HP. The obtained sialon ceramics with fine-grained microstructure show formidably improved superplasticity in the presence of an electric field. The compressive strain rate reaches the order of 10-2 s-1 at temperatures above 1500oC, that is, two orders of magnitude higher than that has been realised so far by any other conventional approaches. The high deformation rate recorded in this work opens up possibilities for making ceramic components with complex shapes through super-plastic forming.
LIST OF PAPERS This thesis is based on the following papers:
I. Zhijian Shen, Hong Peng and Mats Nygren, “The formation of in-situ
reinforced microstructure in α-sialon ceramics: I, with stoichiometric oxygen-
rich compositions.” J. Mater. Res. 17(2) 336-342 (2002).
II. Hong Peng, Zhijian Shen and Mats Nygren, “The formation of in-situ
reinforced microstructure in α-sialon ceramics: II, in the Presence of a Liquid
Phase.” J. Mater. Res. 17(5) 1136-1142 (2002).
III. Hong Peng, Zhijian Shen and Mats Nygren, “The formation of in-situ
reinforced microstructure in α-sialon ceramics: III, static and dynamic
ripening.” J. Mater. Res. in press.
IV. Zhijian Shen, Zhe Zhao, Hong Peng and Nygren, Mats. “Formation of tough
interlocking microstructures in silicon nitride ceramics by dynamic ripening.”
Nature (London, United Kingdom) 417 266 - 269 (2002).
V. Hong Peng, Zhijian Shen and Mats Nygren, “Reaction sequences occurring in
dense Li-doped sialon ceramics: influence of temperature and holding time.” J.
Mater. Chem. 13 2285–2289 (2003).
VI. Zhijian Shen, Hong Peng and Mats Nygren, “Rapid formation and deformation
of Li-doped sialon ceramics.” J. Am. Ceram. Soc. in press.
VII. Zhijian Shen, Hong Peng and Mats Nygren, “Formidable increase of
superplasticity of ceramics in presence of an electric field.” Adv. Mater. 15
(12) 1006-1009 (2003).
Papers not included in this thesis:
VIII. Zhijian Shen, Hong Peng, Pernilla Pettersson, and Mats Nygren, “Self-
reinforced α-sialon ceramics with improved damage tolerance developed by a
new processing strategy.” J. Am. Ceram. Soc. 85(11) 2876-2878 (2002).
IX. Hong Peng, Z. Shen, M.Nygren, “Refinement of the microstructure of self-
reinforced α-sialon ceramics.” Key Eng. Mater. 206-213 1121-1124 (2002).
X. Hong Peng, Zhijian Shen and Mats Nygren, “Fabrication of Li-doped sialon
ceramics by Spark Plasma Sintering.” Key Eng. Mater. in press.
XI. Zhijian Shen, Hong Peng, Jing liu and Mats Nygren, “The conversion from
nano- to microstructure: experimental observations.” J. Eur. Ceram. Soc. in
XII. Hong Peng, Zhijian Shen and Mats Nygren, “In-Situ Reinforced
Stoichiometric α-Sialon Ceramics Prepared by a Novel Sintering Process.” J.
Ceram. Soc. Jpn. in press.
The papers have been reprinted with kind permissions.
TABLE OF CONTENTS ABSTRACT I LIST OF PAPERS III
1. INTRODUCTION................................................................................. 1
1.1 Overview.............................................................................................................. 1 1.1.1 Si3N4 phases ................................................................................................... 1 1.1.2 α-sialon and β-sialon ..................................................................................... 3 1.1.3 Conventional sintering methods .................................................................... 4
1.2 Liquid phase sintering........................................................................................ 6 1.2.1 Classic liquid phase sintering ........................................................................ 6 1.2.2 Liquid-phase sintering of sialon ceramics ..................................................... 8 1.2.3 Densification mechanisms of Si3N4-based ceramics ................................... 10
1.3 Spark Plasma Sintering (SPS)......................................................................... 12 1.3.1 General background..................................................................................... 12 1.3.2 SPS instrument............................................................................................. 13 1.3.3 Consolidation mechanism............................................................................ 14 1.3.4 Features and applications of SPS................................................................. 15
1.4 Properties of Si3N4-based ceramics................................................................. 17 1.4.1 Mechanical properties.................................................................................. 18 1.4.2 Thermal-shock resistance ............................................................................ 18 1.4.3 Superplasticity of ceramics.......................................................................... 19
2. AIM OF THIS THESIS ....................................................................... 22
3. EXPERIMENTAL .............................................................................. 23
3.1 Starting materials ............................................................................................. 23
3.2 Composition design .......................................................................................... 23 3.2.1 Rare-earth stabilised α-sialons .................................................................... 23 3.2.2 Lithium stabilised monolithic α- and duplex α/β-sialon............................ 25 3.2.3 Monolithic β-sialon...................................................................................... 25
3.3 Sintering methods............................................................................................. 26 3.3.1 Hot-press sintering (HP) .............................................................................. 26 3.3.2 Spark Plasma Sintering (SPS) ..................................................................... 26
3.4 Characterisation techniques ............................................................................ 27 3.4.1 X-ray powder diffraction ............................................................................. 27 3.4.2 SEM micrographs ........................................................................................ 27
3.5 Property measurements ................................................................................... 28 3.5.1 Mechanical properties measurements.......................................................... 28 3.5.2 Thermal-shock resistance measurements .................................................... 28 3.5.3 Compressive deformation test ..................................................................... 29
4. REALISING IN-SITU REINFORCED MICROSTRUCTURE THROUGH A NOVEL PROCESSING CONCEPT............................................................. 30
4.1 Hot-pressed stoichiometric α-sialons.............................................................. 30 4.1.1 Crystalline phases present after hot pressing at 1500 oC ............................. 30 4.1.2 Microstructure development ........................................................................ 31 4.1.3 Strategy to obtain elongated morphology.................................................... 33
4.2 New method to introduce extra liquid phase ................................................. 34 4.2.1 A new method to introduce liquid phase ..................................................... 34 4.2.2 Effect of excess oxygen on the phase assemblages obtained ...................... 34 4.2.3 In-situ reinforced microstructures in samples with extra liquid phase........ 35
4.3 Employing a novel sintering technique to prepare sialon ceramics with tailored microstructures ........................................................................................ 37
4.3.1 Enhanced densification by SPS ................................................................... 37 4.3.2 Fast phase transformation ............................................................................ 42 4.3.3 Rapid anisotropic grain growth ................................................................... 44
4.4 Concluding remarks......................................................................................... 46
5. SINTERING KINETICS ..................................................................... 47
5.1 Densification mechanism ................................................................................. 47
5.2 Reaction sequence in fully dense ceramics..................................................... 52
5.3 Grain growth mechanism ................................................................................ 53 5.3.1 Static ripening .............................................................................................. 54 5.3.2 Dynamic ripening ........................................................................................ 55
5.4 Sintering kinetics .............................................................................................. 56
6. PROPERTY EVALUATION .................................................................. 59
6.1 Mechanical properties...................................................................................... 59
6.2 Improved damage tolerance ............................................................................ 60
6.3 Enhanced superplasticity................................................................................. 61 6.3.1 Lithium-stabilised monolithic α-sialon and duplex α/β-composite............ 62 6.3.2 Y-/Yb-doped monophasic α-sialon and β-sialon ........................................ 64 6.3.3 Near net-shape forming ............................................................................... 66
7. PRESENT UNDERSTANDING OF THE SPS PROCESS FOR ENHANCING THE LIQUID PHASE SINTERING................................................................... 68
7.1 Phenomena observed with the SPS apparatus............................................... 68
7.2 Benefits of a rapid heating rate ....................................................................... 69
7.3 Benefits of pulsed DC heating ......................................................................... 69
7.4 Benefits of the use of high pressures ............................................................... 69
7.4 Future work....................................................................................................... 70
8. SUMMARY ....................................................................................... 71
Silicon nitride (Si3N4) based ceramics have been intensively studied for more than
40 years due to their potential application in high-temperature structural
components. They can withstand very harsh environments where metals and
polymers fail. The principal excellent properties of silicon nitride (Si3N4) based
ceramics are: high strength and wear resistance, low density, high decomposition
temperature and oxidation resistance, low coefficient of friction and high resistance
to chemical corrosion1-11.
1.1.1 Si3N4 phases
Silicon nitride occurs in three modifications, the well-known α- and β-Si3N4, and a
newly observed γ-Si3N4 modification12,13. α- and β-Si3N4 have hexagonal structures,
which are built up by corner-sharing SiN4 tetrahedra. They can be regarded as
consisting of layers of silicon and nitrogen atoms in the sequence ABAB... or
ABCDABCD... in α-Si3N4 and β-Si3N4, respectively (see Figure 1.1a and b). The
AB layer is the same in the α and β phases, and the CD layer in the α phase is
related to AB by a c-glide plane. The SiN4 tetrahedra in β-Si3N4 are interconnected
in such a way that tunnels are formed, running parallel with the c axis of the unit
cell. Due to the c-glide plane that relates AB to CD, the α structure contains cavities
instead of tunnels. The cubic γ-Si3N4 is often designated as c modification in the
literature, in analogy with the cubic modification of boron nitride (c-BN). It has a
spinel-type structure in which two silicon atoms each coordinate six nitrogen atoms
octahedrally, and one silicon atom coordinates four nitrogen atoms tetrahedrally, as
seen in Figure 1.1c.
Figure 1.1 Crystal structure stacking model of α-Si3N4, β-Si3N4 and γ-Si3N4: a) The ABCD layer stacking in α-Si3N4, showing that each unit contains two interstitial sites; b) The ABAB layer stacking in β-Si3N4 along the c axis, illustrating the continuous channel along the c axis; c) The spinel structure of γ-Si3N4.
The space group of α-Si3N4 is P31c, with the following lattice parameters:
a = 7.748(1) Å and c = 5.617(1) Å. The corresponding datum for the β modification
is P63 with a = 7.608(1) Å and c = 2.911(1) Å12. The symmetry of γ-Si3N4 is Fd-3m
with a = 7.738(1) Å. Whilst α- and β-Si3N4 can be prepared under normal nitrogen
pressure and hence may be widely used commercially, cubic γ-Si3N4 can only be
prepared in a diamond anvil cell13 or by shock transformation14 at high pressures
1.1.2 α-sialon and β-sialon
α-sialon15 and β-sialon16,17 are two important solid solutions, isostructural with α-
Si3N4 and β-Si3N4, respectively. By substitution of Al-O for Si-N in β-Si3N4, a solid
solution is formed, which was originally named β′-Si3N4, later β′-SIALON, and
nowadays β-sialon. The overall formula of β-sialon is Si6-zAlzOzN8-z, where, the z
value varies continuously from zero to 4.2; and its unit cell contains two “Si3N4”
units. α-sialon is another solid solution based on the α-Si3N4 structure. The formula
of this solid solution is RExSi12-(m+n)Al(m+n)OnN16-n, where RE is a metal ion with a
valence of p+ and m = px. The unit cell of α-sialon comprises four “Si3N4” units,
which are formed by replacement of (m+n)Si-N by m(Al-N) and n(Al-O). There are
two interstitial sites per unit cell in α-sialon, which constrains x to be ≤ 2 in the
formula given above. The added REp+ cations compensate for the valence
discrepancy created by the replacement of m(Si-N) by m(Al-N). Thus, the α-sialon
solid solution range has a two-dimensional extension in the Si3N4–Al2O3·AlN–
REN·3AlN plane located in the Jänecke prism that is commonly used to visualise
the phase relationships among α-sialon and other phases in the RE-Si-Al-O-N
system, as seen in Figure 1.2. In the β-sialon case the replacement of Si-N by Al-O
results in a very small change of the unit cell, because the Si-N and Al-O bond
lengths are very similar; whereas the replacement of (m+n)(Si-N) by m (Al-N) and
n(Al-O) in α-sialon results in a considerable increase of the unit cell size, because
the Al-N bond (1.87 Å) is much longer than Si-N (1.72–1.74 Å).
Figure 1.2 The commonly used Jänecke prism, showing the main phases present in the Si-Al-O-N-RE system.
It is commonly accepted that the β-sialon phase often occurs with a whisker-like
morphology, which promotes the formation of interlocking microstructures. It has
been shown that this type of microstructure yields improved mechanical properties,
e.g. high fracture toughness. For a long time α-sialon was believed to exist only in
an equiaxed shape, until it was experimentally proved in 1995 that elongated grain
morphology can be developed in α-sialon as well18-21. α- and β-sialon ceramics
have been intensively studied during the recent two decades. However, up to now,
only β-Si3N4 and β-sialon have been widely used commercially, mainly because
they are sufficiently hard and can more easily form microstructures with high
fracture toughness values.
1.1.3 Conventional sintering methods
Si3N4 is a highly covalently bonded synthetic material exhibiting very low
diffusivity, so conventional pressureless solid-state sintering methods are not
applicable to producing pure, dense Si3N4-based ceramics. Full density in these
ceramics is achieved by applying pressure and/or by introducing sintering aids to
create a liquid phase that assists the densification.
Dense Si3N4-based ceramics can only be produced, on a technologically interesting
scale, in combination with addition of sintering aids. MgO, Al2O3, AlN, Y2O3 or a
mixture of Al2O3 and Y2O3 are frequently used as sintering aids. The most common
sintering methods used to consolidate Si3N4-based ceramics are the following:
reaction bonding (RB), pressureless sintering (PLS), hot pressing (HP), hot isostatic
pressing (HIP) and gas pressure sintering (GPS). Reaction bonding implies a direct
reaction between Si and N2 during the sintering, but this process often results in
materials with high porosity. It is very difficult to get fully dense Si3N4-based
ceramics without introducing a large amount of liquid phase, using pressureless
Hot pressing is the most established pressure-assisted sintering method, in which
the specimen is placed in a die and an axial pressure is applied by punches. Both the
die and the punches are made of graphite or boron nitride-coated graphite, and the
whole assembly is placed in a furnace. Although the applied pressure promotes the
densification of the specimen, the method has severe limitations when it comes to
preparation of specimens of complex shapes.
In the HIP process the isostatic pressure is applied via a gaseous or liquid medium,
which allows manufacturing of more complicated-shape components in large
quantities. For silicon nitride ceramics, the green bodies are usually coated with a
glass that acts as a gas-tight protective membrane against the gas used as pressure
medium. The furnace is placed in a pressure vessel, and a high-pressurised gas
(normally argon) is pumped into the vessel during the sintering cycle. The entire
set-up is quite complicated and costly, and the glass coating and de-glassing
procedures are also very time-consuming.
Gas pressure sintering implies that the specimens are sintered in an appropriate gas
atmosphere at high pressures, but without using membranes. High nitrogen
pressures are used in connection with gas pressure sintering of Si3N4 based
ceramics, which prevents decomposition of Si3N4, and higher sintering temperatures
can accordingly be applied.
1.2 Liquid phase sintering
Liquid-phase sintering (LPS) is defined as a sintering process that involves liquid
and solid particles. The liquid can be present during the entire sintering process or
during a specific stage of the sintering cycle. There are two basic ways to obtain a
liquid phase: (i) Using mixed powders of differing characteristics; and (ii) Taking
advantage of the interaction between two or more of the components involved. The
liquid can result from the melting of one component or from the formation of a
eutectic liquid. Furthermore, this liquid can be either transient or permanent during
the entire sintering cycle, depending on the solubility relationships as discussed
1.2.1 Classic liquid phase sintering
According to Kingery’s model, the classic liquid-phase sintering process can be
divided into three steps that may in certain cases be partly overlapped23, see Figure
Pores Additives LiquidPores
Base Base Base
Figure 1.3 A schematic drawing showing the microstructural evolution during classic liquid-phase sintering of powder mixtures: I) Rearrangement, II) Solution–precipitation; and III) Microstructure coarsening and solid-state sintering.
The initial stage of classic liquid-phase sintering is a particle rearrangement
process. Rearrangement takes place immediately after the liquid phase forms,
accompanied by rapid partial densification due to the capillary force exerted by the
wetting liquid on the solid particles. The elimination of porosity takes place as the
system minimises its surface energy. The most favourable features for
rearrangement are: (i) A homogeneous distribution of a congruently melting liquid
that wets the particles present; (ii) The solid particles are soluble in the liquid; (iii)
A large solubility ratio. The rate and extent of shrinkage depend upon the viscosity
and quantity of liquid phase formed and on its wetting properties. A relative density
of about 0.65 can be achieved by particle rearrangement. For complete
densification, provided that the amount of liquid phase is less than 35 vol%,
additional sintering processes are necessary.
The second step of this process is termed the solution–reprecipitation step. The
small grains are more soluble than the large ones, and the difference in solubility
establishes a concentration gradient in liquid. Material is therefore transported from
small grains to large grains by diffusion, so that the large grains grow at the expense
of the small during the liquid-phase sintering. This process is known as coarsening,
or static Ostwald ripening (abbreviated as static ripening below)24-26. The major
driving forces for static ripening is the reduction of interfacial energy and the
capillary force. This process relies strongly on two critical steps: dissolution of solid
into the liquid and diffusion through the liquid. If the transport is limited by mass
transfer from the source to the sink, this process is diffusion-controlled; if the
transport is confined by interfacial dissolution or precipitation, the process is
reaction-controlled. Static ripening plays an important role during the solution–
reprecipitation step. It contributes not only to grain growth but also to densification.
The final step of this sintering process is termed the solid-state sintering controlled
step. A solid skeleton is formed, and grain coalescence occurs. The rigidity of the
solid skeleton hinders further rearrangement, although microstructure coarsening
continues by diffusion. In this case, the residual pores will enlarge if they contain
entrapped gas that results in swelling. The densification rate is greatly decreased
during this part of the sintering cycle.
1.2.2 Liquid-phase sintering of sialon ceramics
The densification of silicon nitride based ceramics with sintering additives takes
place via a liquid-phase sintering process5. At high temperatures the introduced
metal oxides react with the oxygen-rich layer (SiO2) that is always present at the
surface of each Si3N4 particle, and with the small Si3N4 particles to form an oxy-
nitride liquid phase, which wets solid particles and allows rearrangement of them.
With increasing temperature, more nitride particles dissolve in the liquid, β-Si3N4 or
sialon phases (if possible) will precipitate when the liquid has become
supersaturated, and this promotes densification by the mechanism of liquid-phase
The mechanism of sintering Si3N4-based ceramics is much more complicated than
that of liquid-phase sintering of hard metals, because intermediate compounds can
be formed and phase transformations occur during the sintering process, which all
consume the liquid phase and/or alter the composition of the liquid9,27-33. Sintering
α-sialon ceramics is thus a complicated process, during which densification, phase
transformation and grain growth normally take place simultaneously. It is not an
easy task to clarify the true mechanism of each stage, e.g. the mechanism governing
The densification of α-sialon in the presence of a liquid phase during the hot-
pressing process can be divided into three steps (frequently overlapped) in terms of
the microstructure development: (i) Particles are rearranged as soon as a melt forms
by reaction between the oxides present on the surfaces of Si3N4 and AlN and the
sintering additives (metal oxides) around 1350oC; (ii) AlN and Si3N4 dissolve into
the liquid as they are wetted by the melt, and the α-sialon grains precipitate when
the liquid has become supersaturated; (iii) Finally, coalescence and grain growth
It has been commonly accepted that the formation of elongated morphology of
Si3N4 grains can be ascribed to the inherent differences in interfacial energy
between various facets of the crystals. However, the relation between the
densification, phase transformation and grain growth during hot pressing of Si3N4-
based ceramics is very complicated, and there are many factors that may influence
the elongation of resultant grains. On the one hand, phase transformation is
expected to enhance the elongation of the grains owing to the enhancement of the
dissolution of α-Si3N4 into the liquid phase. On the other hand, the grain elongation
is inhibited by full densification due to impingement of particles in fully dense
Based on the understanding of the processes given above, the following strategic
steps have been taken with the aim to form a tough interlocking microstructures of
sialon ceramics: (i) Seeding; (ii) Varying the amount and composition of the liquid
phase present; (iii) Promoting the dissolution process by using fine-grained
precursor powders; (iv) Controlling nucleation rate via monitoring the phase
transformations taking place during the sintering process20,38,39. Although it has
been observed that, under high nitrogen pressure, a few grains grow dramatically
fast above 1900oC40,41, and that the growth of anisotropic grains is directly related to
the difference in solubility between small and large grains42, it is generally accepted
that growth of elongated grains is predominantly diffusion controlled43. This implies
that extended holding at high temperature is a necessary requirement to develop a
tough interlocking microstructure.
Microstructure design is crucial for improving the fracture toughness and strength
of silicon nitride-based ceramics, however, the kinetics of the formation of
elongated grains, particularly during or after the phase transformation period, is still
not well understood.
1.2.3 Densification mechanisms of Si3N4-based ceramics
Many investigations have been performed concerning the densification mechanism
of Si3N4-based ceramics. Generally, the Kingery sintering model has been used in
describing the densification results44-51. As mentioned above, the first step is a
rearrangement of the particles that takes place immediately after the liquid phase is
formed and is accompanied by a rapid partial densification due to the capillary
force. The elimination of porosity takes place as the system minimises its surface
energy. Kingery concluded that viscous flow was a dominant mechanism for the
densification at this stage, and used the following equation to describe the time
dependence of the compaction:
∆L/L0 ∝ t 1+y (1-1)
where ∆L/L0 is the relative linear shrinkage, t the holding time at the sintering
temperature and 1+y an exponent somewhat larger than one.
A corresponding equation for diffusion-controlled densification that Kingery
derived for the solution–reprecipitation process, assuming spherical particles, reads:
∆L/L0 = (6⋅k2⋅δ⋅D⋅C0⋅γLV⋅V0/k1⋅R⋅T)1/3⋅ r-4/3⋅ t1/3 (1-2)
where ∆L/L0 is the relative linear shrinkage, k2 a proportionality constant, δ the
grain boundary’s thickness, D the diffusivity of the solid in the liquid, C0 solid
concentration in the liquid, γLV the liquid/solid surface energy, V0 the initial volume,
k1 a constant, R the gas constant, T the temperature, r the initial grain radius and t
the sintering time.
With a grain-boundary reaction-controlled densification:
∆L/L0 = (2⋅ k3⋅k2⋅C0⋅γLV⋅V0/k1⋅R⋅T)1/2⋅ r-1⋅ t1/2 (1-3)
where k3 is a constant.
This implies that, when the shrinkage is proportional to the cube root of the
sintering time, the sintering process is diffusion controlled; and when the shrinkage
is proportional to the square root of the sintering time, it is controlled by grain
For prismatic particles, the shrinkage (∆L/L0) is ∝ t1/5 for diffusion-controlled
densification and (∆L/L0) ∝ t1/3 for grain boundary reaction-controlled densification.
Finally, the third step involves solid-state diffusion process, and diffusion within the
solid is less rapid than that along grain boundaries, so that the diffusion rate
The logarithm of shrinkage is usually plotted versus logarithm of time in order to
determine the densification mechanism. In this type of diagram, the slope of the line
reveals the time exponent. For instance, Hampshire and Jack reported an exponent
of 1/3 for MgO-doped silicon nitride and 1/5 for Y2O3-doped silicon nitride45,52,53,
indicating that the densification is reaction-controlled for MgO-doped silicon nitride
and diffusion-controlled for Y2O3-doped silicon nitride.
Densification during hot pressing of Si3N4-based ceramics has been analysed with
other equations/models than those derived by Kingery. Bowen et al.32,33 used the
Coble equation in a simplified form to describe the obtained densification data in
the MgO-doped silicon nitride system, and thereby to determine the densification
mechanism. The equation used reads:
dρ/dt = 47.5⋅P⋅Db⋅a3⋅W/G3⋅k⋅T (1-4)
where ρ is the relative density, P the applied pressure, Db the grain-boundary
diffusion coefficient and a3 the volume of the rate-controlling species transported;
W is the grain boundary thickness and G the grain size; k is the Boltzmann constant
and T the temperature. It is assumed that the surface energy term may be neglected
in the early densification stage. They found that the densification rate varied with
the applied pressure and the content of MgO additive, confirming that the
densification was controlled by diffusion of Si/N through a magnesium silicate
grain-boundary phase away from the grain-boundary contact region.
That the densification rate during hot pressing is related to the applied stress was
reported by Rahaman and his colleagues 54. With appreciable amounts of liquid
phase, the grain-boundary sliding process is relatively fast and dominates during the
initial part of the shrinkage, but full density is not obtained by this mechanism
alone. In order to yield fully dense samples a solution–reprecipitation process ought
to be operative, and since this process is slower than grain-boundary sliding, the
former process must be the rate-controlling one. The densification rate at a given
density increases linearly with the applied stress. For compositions comprising less
liquid, the grain-boundary sliding process is retarded, and for compositions with
even smaller amounts of liquid the grain-boundary sliding mechanism might
1.3 Spark Plasma Sintering (SPS)
1.3.1 General background
A spark sintering method was investigated and patented in the 1960s and used to
compact metal powders, but due to high equipment cost and low sintering
efficiency it was not put to wider use 55. The concept was further developed during
the mid 1980s to the early 1990s, and a new generation of sintering apparatus
appeared named Plasma Activated Sintering (abbreviated PAS) and Spark Plasma
Sintering (abbreviated SPS). Common to these systems is the use of pulsed direct
current to heat the specimens. These sintering techniques currently attract growing
attention among productions engineers as well as materials researchers. Whether
plasma is generated has not been confirmed yet, especially when non-conduction
ceramic powders are compacted. It has, however, been experimentally verified that
densification is enhanced by the use of a pulsed DC current or field56. This family
of techniques is in academia also named as pulsed electric current sintering
(PECS)57-59 or electric pulse assisted consolidation (EPAC)60. SPS allows
compaction of ceramic and metal powders at low temperature and in short time
Figure 1.4 Basic configuration of a typical SPS system.
1.3.2 SPS instrument
The basic configuration of a SPS unit is shown in Figure 1.4. It consists of a
uniaxial pressure device, where the water-cooled punches also serve as electrodes, a
water-cooled reaction chamber that can be evacuated, a pulsed DC generator,
pressure-, position- and temperature-regulating systems. Figure 1.5 illustrates the
used ON–OFF pulsed direct current during the entire sintering cycle, with a
standard on–off time relation of 12:2. Spark Plasma Sintering resembles the hot
pressing process in several respects, i.e. the precursor powder (green body) is
loaded in a die, and a uniaxial pressure is applied during sintering process.
However, instead of using an external heating source, a pulsed direct current is
allowed to pass through the electrically conducting pressure die and, in appropriate
cases, also through the sample. This implies that the die also acts as a heating
source and that the sample is heated from both outside and inside. The use of a
pulsed direct current also implies that the samples are exposed to a pulsed electric
field during the sintering process.
τon = 6.6ms τon = 40ms
Figure 1.5 The pulsed direct-current used in SPS process.
Figure 1.6 A schematic drawing of the pulsed current that flows through powder particles.
.3.3 Consolidation mechanism
method that is thought be based on momentary
SPS is a pressure-assisted sintering
high-temperature spark (and/or plasma, if present) discharges in the gaps between
powder particles at the beginning of the ON-OFF DC current pulses. It is supposed
that the pulsed current propagates through the powder particles inside the SPS
sintering die, as shown in Figure 1.6. The process inventor also claims that the ON-
OFF DC pulse energising method generates: 1) Spark plasma; 2) Spark impact
pressure; 3) Joule heating; and 4) An electrical field promoting material transfer and
However, in our case when sintering Si3N4-based ceramics, the mechanism as
.3.4 Features and applications of SPS
hat it uses very fast heating rates (up to
described above – the pulse current passing through the powder particles along their
surface – is not applicable, since these ceramics are neither conducting nor semi-
conducting. Whether spark plasma is generated is also doubtful, and the effect of
the spark impact pressure on sintering Si3N4-based ceramics is therefore still
debated. It is true, however, that the applied high-energy pulsed current generates a
pulsed electric field during the entire sintering cycle. This pulsed electric field does
eventually influence sintering process of Si3N4-based ceramics by promoting
material transfer and diffusion of charged species in the liquid phase.
A unique feature of the SPS process is t
600oC/min-1); thus the consolidation rate is greatly enhanced (fully dense materials
are obtained within minutes) and the sintering temperature can be a few hundred
degrees lower than that typically used in conventional sintering processes such as
HP and HIP. Four factors that contribute to the enhanced densification process can
be discerned: (i) The use of rapid heating and cooling rates; (ii) Rapid transfer of
heat because the die itself acts as a heating element; (iii) The application of a
mechanical pressure exceeding that used in the conventional hot-pressing process;
(iv) The use of a pulsed DC current to heat the sample, implying that samples are
also exposed to a pulsed electric field during sintering. It is generally accepted that
application of mechanical pressure promotes the removal of pores and enhances
diffusion. However, it is frequently argued that the improved densification rates
stem mostly from the use of direct current pulses of high energy.
0 20 40 60 260 280 300 320 3400
Figure 1.7 Comparison of typical sintering profiles of sialon ceramics in conventional hot pressing and in spark plasma sintering (SPS).
igure 1.8 SEM micrographs of (Yb+Y)-stabilised sialon specimens of composition (Yb+Y)3512-07, prepared by: HP processing at 1800oC for 4hrs with a heating rate of
FA40oC·min-1 (a) and SPS processing at 1700oC with a holding time of 14 min using a heating rate of 200oC·min-1 (b).
Further advantages of SPS include ease of operation, accurate digital control of
PS has been used to prepare many kinds of materials61,63,66-74, such as advanced
.4 Properties of Si3N4-based ceramics
The microstructure has a significant influence on the characteristic properties of a
sintering profile as well as good reproducibility and reliability. Figure 1.7 shows
two typical temperature-time profiles used in SPS and HP process, respectively,
yielding fully densified Yb/Y-stabilised α-sialon ceramics with similar
microstructures. SEM pictures of these samples are shown in Figure 1.8. A heating
rate of 40 C·min is frequently used in the HP experiment, and the entire sintering
cycle takes more than 300 minutes. In the SPS experiment a high heating rate of
200 C/min is used, and the entire sintering cycle takes less than 20 minutes. This
shows that the densification takes place significantly much faster in the SPS than
that in HP process.
alloy materials, functional gradient materials (FGM), fine ceramics, amorphous
materials, target materials, thermoelectric materials, nano-composites, and it has
also been used for investigation of sintering kinetics. The interest in this sintering
technique is steadily increasing, as manifested by the fact that the number of
publications dealing with this topic has dramatically increased during the last few
material. The microstructure of a material may be tailored by selecting: (i) An
appropriate overall composition; (ii) The characteristics of the precursor powders;
(iii) Type and amount of sintering additives; and (iv) Appropriate sintering
parameters. In Si3N4-based ceramics, the amount, distribution, grain size and
morphology of obtained α and β particles are the decisive factors that determine the
properties of the product.
Table 1.1 Unit cell dimensions, morphologies and mechanical properties of Si3N4-based eramics. c
Unit cell parameter (Å) Mechanical property Morphologya c Hv10 (GPa) K1c (MPa·m-1/2) α-Si3N4 7. ∼20 748(1) 5.617(1) Equiaxed ∼3
(1) (1) Elongated ∼15 ∼6 α-sialon 7.801−7.864 20 2
2 .5 .5
5.679−5.7 Equiaxied Elongated
β-sialon 7.610−7.716 2.911−3.007 Elongated 15–17 5.0–7.0
β-Si3N4 7.617 2.911
.4.1 Mechanical properties
eramics depends on the phase composition because 12,84-86
.4.2 Thermal-shock resistance
of the most important properties of a material
i3N4-based ceramics exhibit high thermal-shock resistance, withstanding
quenching in cold water even from 800–1000oC, whereas other ceramics such as
The hardness of Si3N4-based c
different phases have different hardness values. As shown in Table 1.1 , where
the morphologies and mechanical properties of the major phases in silicon nitride-
based ceramics are listed, the intrinsic hardness of α-sialon (up to 22GPa) is 40%
higher than that of β-sialon and β-Si3N4. High fracture toughness values are found
for ceramics that have interlocking microstructures; thus β-sialon ceramics
consisting of interlocking elongated grains exhibit high fracture toughness, 5–7
MPa·m , whereas α-sialons with equiaxed morphology have low fracture
toughness, between 3 and 3.5 MPa·m . The fracture toughness depends not only on
the grain shape and size but also on the composition of the grain-
Thermal-shock resistance is one
assessing the resistance to weakening or fracture under a rapid change in
temperature, particularly for high-temperature application of structural ceramics. In
monolithic ceramics the thermal shock stems from the fact that the external surface
of ceramic expands or contracts more rapidly than its interior, and this can lead to
cracking or shattering.
ZrO2 or Al2O3 ceramics can only withstand quenching from temperatures ranging
from 200 to 400oC87,88. Various methods have been developed to determine thermal-
shock behaviour. Here, a recently developed indentation-quench technique has been
used to evaluate the thermal shock resistance of three representative sialon
ceramics89,90. This thermal-shock resistance measurement involves four major steps:
(i) Very carefully polishing the surfaces of specimens; (ii) Initiating well-defined
cracks with a Vickers indenter; (iii) Heating the resultant specimens in a vertical
tubular furnace to a pre-set temperature and subsequently quenching the specimens
into a water bath; (iv) Measuring the crack growth and thereafter correlating it with
the temperature difference.
1.4.3 Superplasticity of ceramics
uperplasticity refers to the capability of polycrystalline materials to undergo
microstructural deterioration. Although super-
ally less than approximately 1 µm.
ii) Equiaxed grain morphology. Large shear stresses across the grain
extent that the
igh-energy boundaries. Nano- and/or submicron-sized grains
extensive deformation without any
plastic forming is an established industrial process for many metals91, its
applicability to brittle materials was not demonstrated until the late 1980s. In order
to improve the super-plastic behaviour of a ceramic material, a prerequisite is a
microstructure consisting of fine equiaxed grains, which is stable during the
deformation. The common characteristics of materials with super-plastic behaviour
may be summarised as follows:
i) Small grain size, typic
boundaries are developed during deformation, and to the
grains are non-spherical the grain boundary sliding mechanism becomes
High-energy grain boundaries. Diffusion and sliding proceeds faster
along such h
have boundaries of higher energy than micron-sized grains.
iv) Presence of a second phase. At temperatures where grain-boundary
diffusion and sliding are significant, grains frequently grow fast. A
second phase might be necessary to inhibit grain growth.
v) An amorphous grain-boundary phase/liquid phase (if possible). The
formation of an intergranular liquid/glassy phase, transient or permanent,
is vital for super-plastic deformation in silicon nitride-based ceramics,
because the liquid/glassy phase acts as a lubricant for particle rearrange-
ment and sliding.
Super-plastic deformation of ceramics has attracted technical interest since around
1986, when it was reported that yttria-stabilised tetragonal zirconia polycrystals (Y-
TZP) could be elongated over 100% in tension92-94. Although polycrystalline
tetragonal zirconia is the most intensively investigated material, new developments
have been achieved in Si3N4- and SiC-based ceramics during recent years95. By
reducing the grain size, it turns out that the traditionally brittle ceramics become
ductile96-98. This provides a new method of obtaining ceramic objects with complex
shape, and opens up for new applications of ceramics.
The super-plastic deformation of ceramics occurs mainly via sliding along grain
boundaries; thus the presence of an intergranular glassy phase in conjunction with
ultra-fine-grained microstructures improves the ductility95,99,100. In Si3N4-based
ceramics the deformation progresses very slowly when the coexisting glassy phase
has a high softening temperature and occurs in low concentration97,101,102 and when
the constituent grains possess a fibrous morphology103. To enhance the ductility of
Si3N4-based ceramics, in particular at lower temperatures, compacts that contain
equiaxed submicron-sized grains have been prepared by: (i) Applying a low-
temperature sintering procedure104; (ii) Adding grain-growth inhibitors, e.g. SiC
particles100; (iii) Using β-Si3N4 powder, because this precursor seems more resistant
to grain growth101.
Si3N4-based ceramics with fine, equiaxed morphology show reduction in both
fracture strength and fracture toughness at room temperature, but they are the ones
that exhibit super-plastic behaviour at high temperature. The ductility of this type of
ceramics is strongly temperature dependent; it increases with increasing temperature
up to a certain critical temperature (Tc). Above Tc the ductility is hindered because
the accelerated grain growth induces strain hardening. Strain rates of the order 10-4
s-1 are thus obtained under a compressive stress of 40–50 MPa at temperatures
around 1500oC. Attempts have been made to reduce the viscosity of the grain-
boundary glassy phase even further via compositional adjustment in order to lower
its softening temperature102. However, the resistance to creep and corrosion is
thereby decreased, i.e. properties that are vital for materials intended for high-
temperature applications are then sacrificed.
2. Aim of this thesis
The main work of this thesis has been focused on sintering and characterisation of
sialon ceramics with different metal oxides as sintering additives. SPS is the
principal sintering method that has been used to ensure full densification, while a
conventional sintering process such as HP has also been applied for the sake of
comparison. The main work includes the following aspects:
The effect of sintering additives on sintering process during conventional
HP processing, particularly their influence on grain growth.
Introducing an extra liquid phase that is thermodynamically compatible
with sialon phases by using a new approach, namely increasing the O/N
ratio in the general formula RExSi12-(3x+n)Al3x+nOnN16-n whilst keeping the
RE, Si, and Al proportions constant.
Investigation of sintering kinetics under SPS conditions, focusing on
densification, phase transformation and grain growth, respectively.
Tailoring the microstructures of sialon ceramics.
Improving super-plastic properties of silicon nitride-based ceramics to
yield complex shape components.
3.1 Starting materials
The starting powders were commercial α-Si3N4 (UBE, SN-10E), β-Si3N4 (SN
P21FC), Al2O3 (Alcoa, SG30), AlN (HC Starck–Berlin, Grade C), Li2CO3 (in the
Li-stabilised sialon system) and RE2O3 where RE = Y, Nd, Sm, Dy, and Yb
(Johnson Matthey Chemicals Ltd.). When calculating the overall compositions,
corrections were made for the small amounts of oxygen present in the Si3N4 and
AlN raw mixtures. The starting materials, in batches of 50 g, were ball milled in
water-free propanol for 24 hrs, using sialon milling media, and then dried in an
oven at 80oC for 24 hrs. If not otherwise stated, α-Si3N4 (UBE, SN-10E) was used
as silicon nitride precursor in this work.
3.2 Composition design
3.2.1 Rare-earth stabilised α-sialons
α-sialon samples with two slightly different stoichiometric compositions were
investigated, namely x = 0.35, n = 1.2 for RE = Y, Yb, Sm, Dy and an equimolar
mixture of Y and Yb, and x = 0.35, n = 1.0 for RE = Nd in the general formula
RExSi12-(3x+n)Al3x+nOnN16-n. The two compositions, referred to ARE3512 and ANd-
3510 below, respectively, are located close to the oxygen-rich boundary of the α-
sialon phase region facing the β-sialon line.
The oxygen content of ARE3512 is 5.16 eq% in the starting overall composition.
By fixing the cation ratio of this composition and increasing the oxygen content
from 5.16 to 15 eq%, a series of powder mixtures were prepared along the A–B line
located slightly above the α-sialon plane in the Jänecke prism of the RE-Si-Al-O-N
system, as shown in Figure 3.1.
Figure 3.1 A schematic representation of the Jänecke prism of RE-Si-Al-O-N systems. The compositions investigated in this thesis are located along the line A-B.
These compositions are named AY3512-ZZ, AYb3512-ZZ and A(Y+Yb)3512-ZZ
below, where thus A(Y+Yb)3512-ZZ represents samples with Yb and Y in equal-
molar proportions as stabilising agent, and with ZZ representing the oxygen content
of the sample expressed in eq%. The ZZ value of the selected basic composition,
RE0.35Si9.75Al2.25O1.20N14.80 (ARE3512), is thus 5.16, and powder mixtures with
ZZ = 07, 08, 09, 10, 11, 12, 13, and 15 were also prepared. Table 3.1 shows the
systematic labels of the rare-earth stabilised samples prepared.
Table 3.1 Systematic labelling of the α- and β-sialons investigated based on a starting composition of RExSi12-(3x+n)Al3x+nOnN16-n, where x = 0.35 and n = 1.2.
Sample O eq% Remarks General formulae
ARE3512(-05) 5.16 RE=Y, Yb, Y+Yb, DY, Sm RE0.35Si9.75Al2.25O1.20N14.80 ARE3512-07 7.0 RE=Y, Yb RE0.35Si9.75Al2.25O1.64N14.50 ARE3512-10 10.0 RE=Y, Yb RE0.35Si9.75Al2.25O2.34N14.04 ARE3512-15 15.0 RE=Y, Yb RE0.35Si9.75Al2.25O3.51N13.26 A(Yb+Y) 3512-ZZ ZZ=07, 08, 09, 10, 11, 12, 13, and 15 Yb0.175Y0.175Si9.75Al2.25OaNb*
* a and b are calculated according to the O eq% by following the equations: 2a/(2a+3b) = O eq% and 2a + 3b = 1.2·2 + 14.8·3 = 46.8.
3.2.2 Lithium stabilised monolithic α- and duplex α/β-sialon
Lithium-stabilised sialon samples with overall compositions either corresponding to
an α/β-sialon composite with m = 0.5 and n = 2.0 or to a monophasic α-sialon with
m = 1.0 and n = 2.5 in the general formula LixSi12-(m+n)Alm+nOnN16-n were
investigated. These two compositions are labelled Li0520 and ALi1025,
Both α-Si3N4 (UBE, SN-10E) and β-Si3N4 (SN P21FC) powders were used as
precursors in connection with the preparation of the duplex composite α/β-sialon
(Li0520). The resultant samples were labelled ALi0520 and BLi0520, with initial A
and B representing α- and β-Si3N4 as precursors, respectively. The selected
composition is located in the duplex α/β-sialon phase region, implying that the α-
and β-sialon phases ought to form in conjunction with some glassy phase when
thermodynamic equilibrium is approached.
Based on the monophasic α-sialon composition ALi1025, by slightly increasing the
oxygen content to 17 eq% while keeping the cations constant, a duplex α/β-sialon
with overall composition LiSi8.5Al3.5O3.9N12.6 was derived and labelled ALi1025-17.
This composition yields a sialon composite containing ∼54% α- and ∼46% β-
3.2.3 Monolithic β-sialon
One monolithic β-sialon with composition Y0.01Si1.91Al0.215O0.166N2.66, labelled
G20B06, was designed for comparison in investigating the grain growth kinetics
and super-plastic behaviour.
3.3 Sintering methods The precursor powder mixtures were consolidated using conventional hot pressing
and/or SPS processing. The SPS process was used as principal sintering method for
consolidating sialon ceramics in this work, and for comparison, the HP process was
used to densify appropriate samples and to perform super-plastic deformation
3.3.1 Hot-press sintering (HP)
Hot pressing was performed in a graphite-heated furnace (Thermal technology,
Germany) in protecting nitrogen atmosphere. The dried powders of RE-stabilised
sialon ceramics were compacted to pellets with a diameter of 18 mm, which were
then HPed at 32 MPa in nitrogen atmosphere in a graphite resistance furnace. A
two-step sintering procedure was applied, i.e. the samples were first heated to
1500oC at a rate of 15oC·min-1 and held there for one hour; they were then further
heated to the final sintering temperature, 1800 or 1900oC, at a rate of 40oC·min-1
and held there for 4 hrs. After sintering, the samples were allowed to cool inside the
furnace at a rate of ∼50oC·min-1. To obtain fully dense sialon ceramics in HP, a
prolonged dwelling time is necessary, making it difficult to control the morphology
of obtained specimens.
3.3.2 Spark Plasma Sintering (SPS)
The SPS process was carried out in vacuum in a spark-plasma sintering apparatus,
Dr. Sinter 2050 (Sumitomo Coal Mining Co. Ltd. Japan). The precursor powders
were loaded in a cylindrical carbon die with an inner diameter of 20 mm. The
samples were heated by passing a pulsed DC current through the pressurised die,
i.e. using the die also as a heating source. The final sintering temperature was set
between 1450 and 1830oC, with or without holding. The temperature was
automatically raised to 600oC over a period of 3 min, and from this point it was then
monitored and regulated by an optical pyrometer focussed on the surface of the die.
If not otherwise stated, the heating rate was 200oC·min-1 when sintering RE-
stabilised sialon, and 100oC·min-1 in Li-stabilised systems; a pressure of 50 MPa
was maintained throughout the sintering cycle. The set-up allows a cooling rate of
> 350oC·min-1 in the temperature range 1830–1000oC.
3.4 Characterisation techniques
3.4.1 X-ray powder diffraction
X-ray powder diffraction (XRD) was used for phase identification. The X-ray
patterns were recorded in a Guinier–Hägg camera using monochromatic CuKα1
radiation. Small amounts of Si were used as internal standard, and the patterns were
evaluated by means of the SCANPI system. The unit cell parameters of the
recognised crystalline phases were refined with the PIRUM computer software105.
The obtained cell parameters were used to calculate the x value of the α-sialon and
the z value of the β-sialon in their general formulae according to the empirical
expressions given by Shen et al106,107 and Ekström et al108:
a = 7.752+0.139xa; c = 5.620+0.153xc; x = (xa+xb)/2 (3-1)
for the α phase;
a = 7.603+0.0297za; c = 2.907+0.0255zc; z = (za+zc)/2 (3-2)
for the β phase.
The amounts of α- and β-sialons in the obtained specimens were estimated by
comparing the intensities of the two strongest peaks yielded by each phase, (102)
and (210) for α-sialon and (110) and (210) for β-sialon.
3.4.2 SEM micrographs
Polished and/or fractured surfaces of all specimens were examined in a scanning
electron microscope (SEM, Jeol JSM880), equipped with an energy-dispersive
spectrometer (EDS, LINK ISIS). In order to obtain the best contrast between
different phases, the micrographs were recorded in back-scattering electron mode
(BSE) for polished surfaces. The α-sialon and RE-enriched intergranular phases
show medium grey and bright contrasts, respectively, while β-sialon and sialon
polytypoids (if present) appear with dark black contrast. Fracture surfaces of the
prepared samples of lithium-stabilised sialons were etched in a molten mixture of
KOH and KNO3 for 1–3 minutes before SEM examination.
The average size of the 10 largest grains that could be clearly distinguished in each
SEM micrograph of the fractured or polished surfaces was measured. Five
randomly selected, equally magnified areas of each sample were recorded and used
for the grain size measurements. The sizes of selected grains were determined by
means of an image analysis program (Image tool, UTHSCSA).
3.5 Property measurements
The bulk densities of the sintered samples were determined based upon the Archi-
medes principle. Before studying the mechanical properties and microstructures,
the specimens were carefully polished by standard diamond polish technique down
to 1 µm finish.
3.5.1 Mechanical properties measurements
Hardness and fracture toughness were measured with a Vickers diamond pyramid
indenter by applying a load of 98 N, and were calculated by both Anstis109 and
3.5.2 Thermal-shock resistance measurements
The thermal shock resistance was examined in a vertical tubular furnace heated to a
pre-set temperature, using fully dense cylindrical samples with a diameter of 12 mm
and a thickness of ∼4 mm. Well-defined cracks were initiated with a Vickers
indenter on the very carefully polished surfaces of samples. Four indents were made
on each sample, each indent generating four cracks; a total of sixteen cracks were
thus initiated on each sample. The sample was hoisted into the furnace and was
thermally equilibrated for 20 min and subsequently quenched into a 90oC water
bath. Thereafter the crack growth at each temperature step was measured and
correlated with the temperature difference.
3.5.3 Compressive deformation test
The compressive deformation tests were carried out both in the SPS apparatus and
in a conventional hot-pressing chamber. Fully densified cylindrical samples with a
diameter of 12 mm and a height of ∼6 mm were loaded in a graphite die with inner
diameter 20 mm, and were deformed under a uniaxial compressive stress applied
via the graphite punches of the pressure die. A constant heating rate of 40oC·min-1
was applied during the entire deformation cycle. A load corresponding to an initial
stress of 40 MPa was applied at room temperature and was held constant during the
entire deformation process.
4. Realising in-situ reinforced microstructure through a novel processing concept
4.1 Hot-pressed stoichiometric α-sialons
Monophasic α-sialon with stoichiometric composition ARE3512, i.e.
RE0.35Si9.75Al2.25O1.20N14.80, where RE = Y, Yb, Dy, and Sm, or ANd3510,
Nd0.35Si9.95Al2.05O1.00N15.00, were prepared from α-Si3N4 precursor powder using
conventional hot pressing in protecting nitrogen atmosphere.
4.1.1 Crystalline phases present after hot pressing at 1500 oC
Crystalline phases present after hot pressing at 1500oC for 1 hr are listed in Table
4.1, which reveals that the reactions leading to the formation of α-sialon are rather
slow at this temperature, as manifested by the large amount of the nitride
precursors, α-Si3N4 and AlN still remaining in the compacts. In addition, a
nitrogen-rich melilite phase, RE2Si3-xAlxO3+xN4-x (labelled M’ below), formed in
large amounts in the Nd-, Sm- and Dy-doped samples. In the Y-doped samples
there appear small amounts of M’ together with larger amounts of the oxide phase,
Y3Al5O12 (YAG). No crystalline intermediate phase was observed in the Yb-doped
sample. The α-sialon/α-Si3N4 ratio was found to be 0 and 0.10 in the Nd- and Sm-
doped samples, respectively, whereas this ratio ranged from 0.20 to 0.30 for the
other RE elements used. This confirms that the formation of α-sialon is retarded in
the Nd- and Sm-doped samples due to the formation of M’ phase.
4.1.2 Microstructure development
Fully dense compacts were obtained after hot pressing at 1800 and 1900oC for 4
hrs, and the only crystalline phase in these compacts was α-sialon, according to the
X-ray powder patterns, with the exception of Nd-, and Sm-doped samples where
trace amounts of β-sialon grains were found. As shown in Figure 4.1, all samples
contained a very small amount of a residual intergranular amorphous phase,
confirming that the overall compositions of the present samples are indeed located
on the oxygen-rich boundary of the single-phase α-sialon region.
Table 4.1 Crystalline phase assemblages in RE-doped α-sialons with stoichiometric composition after hot pressing for 1 hr at 1500oC
X-ray peak intensity*
Compositions α-Si3N4 AlN α sialon Melilite Garnet α’/α#
ANd3510 vs m s 0
ASm3512 vs m vw vs 0.10
AY3512 vs m w w s 0.17
ADy3512 vs m w s 0.30
AYb3512 vs m w 0.20
* Intensity decreases in the order vs > s > m > w > vw. # Intensity ratio of (102) peaks from α-sialon /α-Si3N4.
Elongated α-sialon grains formed in large amounts in Nd- and Sm-doped samples,
less abundantly in Y- and Dy-doped ones, and not at all in the Yb-doped one. The
grain growth is obviously enhanced at the higher temperature, as coarser grains
and/or grains with higher aspect ratios are formed at 1900 than at 1800oC, see
Figure 4.1. The Nd- and Sm-doped samples prepared at 1900oC exhibit a clearly
bimodal grain size distribution, i.e. they contain very large elongated grains up to a
few tens of micrometers in length, embedded in a matrix consisting of sub-
micrometer sized equi-axed grains. The Y- and Dy-doped samples prepared at
1900oC contain much coarser grains than found in compacts prepared at 1800oC,
but most of these grains have equi-axed morphology. However, the Yb-doped
sample prepared at 1900oC still has a microstructure consisting of only small equi-
axed grains with very narrow size distribution.
Figure 4.1 Back-scattered SEM micrographs of the samples with stoichiometric overall ARE3512 compositions, hot-pressed at 1800oC for 4 hours (a), and at 1900oC for 4 hours (b). The microstructure of the Y-doped sample resembles that of the Dy-doped one.
In the Nd-, Sm-, and Dy-doped α-sialon systems, a number of intermediate phases
form during heating, but they decompose near the final sintering temperature that
provides the system with the transient liquid necessary for elongated grain growth.
Because only a small amount of liquid forms at lower temperatures, the number of
α-sialon nuclei formed in this temperature region is limited, which explains why
elongated α-sialon grains are readily formed in these systems. In the Yb-doped
system almost no transient phases are formed at intermediate temperatures,
implying that more α-sialon nuclei form in a narrow temperature interval and,
accordingly, it becomes much more difficult to obtain elongated α-sialon grains.
4.1.3 Strategy to obtain elongated morphology
Using conventional hot pressing, Y- and Yb-stabilised monophasic α-sialons with
stoichiometric composition, exemplified by AY5312 and AYb3512 (see Table 3.1),
retain the equi-axed morphology even at a temperature as high as 1900oC. In such
systems, due to the absence of the formation and subsequent decomposition of
intermediate phases during sintering, conditions suitable for elongated grain growth
has never been established. To obtain elongated morphology, a condition of higher
temperature and/or extra liquid has to be satisfied. However, two facts are worth to
consider: (i) Severe decomposition of Si3N4-based phases starts above 1900oC if an
overpressure of N2 is not applied; and (ii) Introducing too large amount of extra
liquid that finally remains as a permanent glass phase at grain boundaries will
deteriorate high-temperature properties of the formed ceramics.
Consequently, to resolve the difficulty in developing elongated grain morphology in
monophasic α-sialon ceramics, we propose two new concepts: (i) Developing a new
method of introducing a small amount of liquid phase that is thermodynamically
compatible with the α-sialon phase; and (ii) Employing novel sintering techniques,
which should provide possibilities to prevent exhausting the transient liquid during
heating and momentarily promote the formation of a large concentration of a
transient liquid at the temperature suitable for grain growth.
4.2 New method to introduce extra liquid phase
4.2.1 A new method to introduce liquid phase
Simply supplying one or more oxide additive(s) or a pre-designed liquid component
to a monophasic α-sialon composition will most probably shift the composition
away from the α-sialon forming region, implying that one or more crystalline
phase(s), e.g. β-sialon, melilite or garnet, may be formed besides an amorphous
intergranular phase107. In the present work, a small amount of liquid phase that is
thermodynamically compatible with α-sialon was introduced by raising the oxygen
content of an already oxygen-rich α-sialon composition, i.e. by increasing the O/N
ratio in RExSi12-(3x+n)Al3x+nOnN16-n while keeping the RE, Si and Al contents
unchanged, see §3.1. Thus, for instance, based on a stoichiometric composition of
RE0.35Si9.75Al2.25O1.20N14.80, a series of sialons with varied oxygen equivalent
percentages of 7 %, 8%, 9%, 10%, 11%, 12% and 15% were prepared, where RE
represents Y and Yb in equi-molar proportion as seen in Table 3.1.
4.2.2 Effect of excess oxygen on the phase assemblages obtained
Densities, phase assemblages, and unit cell dimensions of α- and β-sialon phases
present in obtained specimens by hot-pressing at 1800oC for 4 hrs are listed in Table
4.2. It is evident that the crystalline phase assemblages in the compacts change
from containing only the α-sialon phase to containing mainly β-sialon via the
formation of duplex α/β-sialon compacts when the overall oxygen equivalent
percentage of the samples increases from 5.16 eq% in RE0.35Si9.75Al2.25O1.20N14.80 to
15.0 eq% in RE0.35Si9.75Al2.25O3.51N13.26. A detailed phase analysis study of the
A(Y+Yb)3512-ZZ sample series revealed that the upper limit of the oxygen content
for obtaining monophasic α-sialon is around 7.0 eq%. Compacts containing α- and
β-sialon phases were obtained between 7.0 and 12.5 eq% oxygen, and above 12.5
eq% the only crystalline phase present was β-sialon. It should be noted that the unit
cell dimensions of the α- and β-sialon phases are similar in all samples. Besides α-
sialon and β-sialon (if present) phases, no other crystalline phase was identified.
The amount of residual intergranular amorphous phase, which is expected to be
liquid at the sintering temperature, increases with increasing overall content of
oxygen, as revealed by the SEM pictures shown in Figure 4.2.
Table 4.2 Phase assemblages, unit cell dimensions and densities of specimens obtained by hot pressing at 1800oC for 4 hrs. Phase content (%) α sialon β sialon Density
Sample label α-sialon β-sialon a(Å) c(Å) a(Å) c(Å) zavg. (g/cm3)
AY3512 100 0 7.8117 5.6918 3.26
AY3512-07 100 0 7.8051 5.6912 3.25
AY3512-10 35 65 7.8114 5.6941 7.6248 2.9320 0.86 3.25
AY3512-15 0 100 7.6338 2.9320 1.00 3.20
AYb3512 100 0 3.41
AYb3512-07 100 0 7.8115 5.6918 3.43
AYb3512-10 55 45 7.8115 5.6920 7.6387 2.9279 1.01 3.38
AYb3512-15 0 100 7.6351 2.9333 1.06 3.30
A(Yb+Y)3512 100 0 7.8098 5.6897 3.31
A(Yb+Y)3512-07 100 0 7.8095 5.6917 3.32
A(Yb+Y)3512-08 80 20 7.8076 5.6897 7.6333 2.9295 0.95 3.33
A(Yb+Y)3512-09 64 36 7.8105 5.6916 7.6340 2.9293 0.96 3.32
A(Yb+Y)3512-10 49 51 7.8112 5.6941 7.6359 2.9307 1.02 3.32
A(Yb+Y)3512-11 25 75 7.8099 5.6920 7.6323 2.9280 0.91 3.31
A(Yb+Y)3512-12 8 92 7.8086 5.6906 7.6340 2.9290 0.95 3.30
A(Yb+Y)3512-13 0 100 7.6338 2.9299 0.97 3.25
A(Yb+Y)3512-15 0 100 7.6338 2.9319 1.01 3.26
4.2.3 In-situ reinforced microstructures in samples with extra liquid phase
Without addition of an extra liquid phase, the α-sialon grains possess an equiaxed
morphology with an average grain size around 1 µm when hot-pressed at 1800oC
for 4 hrs, as shown in Figure 4.1 and Figure 4.2a. The Y-, Yb- or (Y+Yb)-doped
specimens had very similar microstructures. In contrast, the presence of an extra
liquid phase aids the formation of grains with elongated morphology, as revealed by
the SEM picture of (Yb+Y)-doped specimens shown in Figure 4.2b–d. There is a
clear tendency for more elongated grains of both the α- and β-sialon phases to form
with increasing overall oxygen content. One can also note that the average grain
size decreases with increasing amount of liquid present, and that the elongated β-
sialon grains are thinner than those of α-sialon.
Figure 4.2 Backscattered SEM micrographs of (Y+Yb)-stabilised sialon ceramics based on the ARE3512-ZZ composition, hot pressed at 1800oC for 4 hrs and containing (a) 5.1 eq%, (b) 7 eq%, (c)10 eq% and (c) 15 eq% oxygen. As revealed by Figure 4.2, a slight increase of the oxygen content from the
stoichiometric value 5.16 eq% to the non-stoichiometric one 7.0 eq% caused a small
amount of an extra liquid phase to be introduced while α-sialon still remains the
only crystalline phase. The amount of liquid formed corresponds to ∼3 vol%
according the quantitative image analysis. An in-situ reinforced microstructure
containing elongated grains (up to ten micrometers in length) embedded in a matrix
consisting of sub-micron sized equiaxed grains was found in all specimens of this
overall composition, whether or not Y, Yb, or a mixture of Y and Yb was used as
stabilising agent. The number of elongated grains and their sizes vary with the type
of stabilising ion used. Thus, more elongated grains with wider cross-sections were
formed in the (Y+Yb)-doped specimen than in those containing Y or Yb alone (see
Figure 4.2b and Figure 4.3). A quantitative analysis reveals that the mean widths of
the elongated grains are 1.3, 1.5, and 1.8 µm in the Y-, Yb-, and (Y+Yb)-doped
Figure 4.3 Backscattered SEM micrographs of monophasic α-sialon ceramics, hot pressed at 1800oC for 4 hrs, with starting compositions AY3512-07 (a) and AYb3512-07 (b).
4.3 Employing a novel sintering technique to prepare sialon ceramics with
4.3.1 Enhanced densification by SPS
The temperature dependence of the normalised shrinkage, the phase assemblages
and the grain sizes of SPS consolidated specimens of composition AYb3512 are
presented in Figure 4.4. The densification starts at ~1300oC and is complete at
~1550oC without holding. The entire densification takes less than 1.5 min,
demonstrating the very rapid densification feature of the SPS process. As shown in
Chapter 3, a transient liquid phase is formed at the intermediate sintering stage in
samples of overall ARE3512 composition. This liquid phase is more or less totally
consumed at the end of the sintering process, whereas approximately 3vol% of an
extra liquid/glass remains after sintering samples based on overall composition
1200 1300 1400 1500 1600 1700 1800 1900
30 α-sialon content Shrinkage
Grain width Grain length
Figure 4.4 Shrinkage, grain size and phase content plotted versus temperature for SPS-consolidated samples based on the AYb3512 composition.
1000 1200 1400 1600 1800
Figure 4.5 Normalised shrinkage curves recorded during SPS processing of specimens based on the compositions A(Yb+Y)3512 and A(Yb+Y)3512-07.
The corresponding normalised shrinkage curves of the specimens based on the
stoichiometric composition A(Yb+Y)3512 and the non-stoichiometric composition
A(Yb+Y)3512-07 are shown in Figure 4.5. In both cases the densification starts at
∼1250oC but it completes at different temperatures, namely ∼1550 oC and ∼1600 oC
for compositions A(Yb+Y)3512-07 and A(Yb+Y)3512, respectively. It thus appears
that the presence of an extra liquid phase improves the densification. Similar rapid
densifications were also observed in other RE-stabilised sialon ceramics, e.g.
ADy3512, ASm3512 and ANd3510 (see Table 3.1) when the SPS process was
applied. It can be noted that specimens hot-pressed at 1500oC for 1 hr did not
800 1000 1200 1400 1600 1800
1000 1200 1400 1600 1800-0.002
Figure 4.6 Normalised shrinkage recorded during SPS processing of the specimen based on the composition AY3512-10. Shown in the inset is the shrinkage rate versus the sintering temperature.
Figure 4.6 shows the shrinkage curve recorded for a α/β-sialon composite of overall
composition AY3512-10, where the shrinkage starts at ∼1200oC and ends at
1500oC, using a heating rate of 200oC⋅min-1. Two shoulders are observed in this
shrinkage curve. We interpret these two shoulders, marked by the arrows at ∼1200
and ∼1350oC, respectively, as onsets of the formation of two types of liquid phase.
The insert shows the shrinkage rate during densification, and the curve comprises
two peaks, which are assumed to correspond to these two types of liquid phase. The
former signals the formation of an oxide-based liquid just above the lowest eutectic
temperature in the Y2O3–SiO2–Al2O3 system, and the latter implies formation of a
nitrogen-containing liquid just above the lowest eutectic temperature in the Y–Al–
Si–O–N system. The time difference between the formations of two liquid phases is
less than 1 min. This implies that a non-equilibrium liquid is formed during the
rapid sintering process, and its presence accelerates the densification, as the
viscosity of concomitant liquids is expected to be comparatively low. The densities,
morphology and crystalline phase assemblages of the formed phase(s) in SPS
consolidated specimens prepared in the temperature interval 1400oC to 1700oC are
listed in Table 4.3. In this particular case, fully dense samples were obtained already
at a temperature of ∼1450oC, and the entire densification process was completed
within 2 min.
Table 4.3 Densities, morphologies and crystalline phase assemblages for α- and β-sialon phase formed in specimens of composition AY3512-10, SPS consolidated at different temperatures without holding.
Crystalline assemblages (%) Temperature ( oC)
Morphologyα-S3N4* β-sialon α-sialon
1400 2.95 Equiaxed 100 0 0 1450 3.28 Equiaxed 66 11 23 1500 3.26 Equiaxed 59 13 28 1600 3.25 Equiaxed 13 36 51 1650 3.25 Elongated 0 51 49 1700 3.24 Elongated 0 51 49
* Un-reacted α-S3N4 Specimens of overall compositions ALi1025 and ALi1025-17 (see §3.2.2) were
fully densified at T ≥ 1450oC and 1400oC respectively, without holding and using a
heating rate of 100oC⋅min-1, as seen in Figure 4.7. The sintering shrinkage starts at
∼1100oC and stops at ∼1450 and ∼1400oC for compositions ALi1025 and ALi1025-
17, respectively, implying that the entire densification process takes only 3–3.5 min.
Two shoulders, marked by the arrows at ∼1100 and ∼1300oC, were also observed in
the shrinkage curves of these two compositions. This implies that the oxide-based
liquid formed at the lowest eutectic in the Li2O–SiO2–Al2O3 system, and the
nitrogen-containing liquid formed at the lowest eutectic in the Li-Si-Al-O-N
system. The ALi0520 and BLi0520 specimens (see §3.2.2) exhibit similar rapid
densification, and fully dense samples were obtained at 1450 and 1500oC,
respectively. The densities, crystalline phase assemblages and unit cell parameters
of the α/β-sialon phases formed in these two compacts are given in Table 4.4.
1000 1100 1200 1300 1400 1500
Figure 4.7 The shrinkages recorded in SPS apparatus during densification of the specimens based on compositions ALi1025 and ALi1025-17, plotted versus temperature. Table 4.4 Densities, crystalline phase assemblages and unit cell parameters for α- and β-sialon phases formed in specimens ALi0520 and BLi0520 in the SPS apparatus at different temperatures, without holding.
Sintering Density Phases (%)* α- sialon β- sialon Sample temperature (g/cm3) α′ β′ α/β a (Å) c (Å) xaverage a (Å) c (Å) z average ALi0520 1450oC 3.14 19 0 81 7.8443 5.6898 0.48
1600oC 3.13 100 0 7.8135 5.6775 0.42 1650oC 3.13 76 24 7.8099 5.6769 0.40 7.6563 2.9403 1.55 1700oC 3.04 47 53 7.8075 5.673 0.38 7.6586 2.9407 1.60
BLi0520 1500oC 3.14 15 0 85 1600oC 3.13 41 25 34 7.8277 5.6913 0.51 7.6694 2.944 1.84 1650oC 3.13 36 44 20 7.8212 5.6878 0.48 7.6588 2.9435 1.66 1700oC 3.06 41 59 0 7.8125 5.6736 0.40 7.6528 2.9400 1.47
*α′ and β′ represent α-and β-sialon, respectively; α/β are the remained α- and β-Si3N4 in Ali0520 and BLi0520, respectively.
The shrinkage curves given in Figures 4.4-4.7 show a similar trend during the
densification process, i.e. shrinkage is very rapid as soon as it is thermally activated.
Two shoulders were observed in the shrinkage curve and these two shoulders signal
two types of liquid phase appearing during the densification process.
Table 4.5 Preparation conditions, phase assemblages, unit cell dimensions and mechanical properties of specimens obtained in the SPS apparatus at different temperatures, without holding. Samples Temperatures α-sialon Hv10 K1c
(oC) a (Å) c (Å) α (%)∗ (GPa) (MPa.m1/2)
AYb3512 1550 7.8175 5.6972 76.4 20.2±0.2 3.9±0.2
1600 7.8137 5.6875 90.0 20.4±0.2 3.6±0.2
1650 7.8078 5.6833 100 20.6±0.2 3.8±0.2
1700 7.8062 5.6826 100 19.7±0.2 4.2±0.1
1750 7.8063 5.6846 100 19.9±0.2 5.2±0.3
1830 7.8085 5.6865 100 19.6±0.2 5.3±0.2
AYb3512-07 1500 7.8352 5.7124 72.7 19.9±0.2 3.5±0.2
1600 7.8113 5.6978 92.0 19.8±0.2 3.7±0.1
1650 7.8079 5.6883 100 20.2±0.2 3.9±0.2
1700 7.8065 5.6896 100 20.1±0.2 4.4±0.1
1750 100 19.6±0.2 6.3±0.2
1800 100 20.0±0.2 6.2±0.3
A(Yb+Y) 3512-07 1550 7.8185 5.6986 79.4 18.7±0.2 3.5±0.1
1600 7.8152 5.6913 100 19.6±0.1 3.6±0.2
1700 7.8117 5.6887 100 20.3±0.2 4.3±0.2
1750 100 19.9±0.1 5.1±0.1
1830 100 20.1±0.2 5.4±0.1
* The additional crystalline phase is un-reacted Si3N4.
4.3.2 Fast phase transformation
The temperature dependence of the α-sialon content in samples AYb3512,
AYb3512-07 and A(Yb+Y)3512-07 is shown in Table 4.5. It is obvious that the α-
sialon phase is the only crystalline phase when thermodynamic equilibrium is
reached, while at the lowest sintering temperatures applied the transformation from
α-Si3N4 to α-sialon is not complete even though full densification is achieved.
Thus, at 1550oC the A(Yb+Y)3512-07 and AYb3512 samples are both fully
densified, but contain, according to the X-ray analysis, ~20 % and ~23.4 % un-
reacted α-Si3N4, respectively. The formation of α-sialon is not completed in fully
densified compacts until the sintering temperature is increased to 1600oC and
1650oC for compositions A(Yb+Y)3512-07 and AYb3512, respectively. Taking
into account that the time spent in increasing the temperature from 1550 to 1650oC
is approximately 0.5 min, it appears clearly that the phase transformation progress is
also very fast in the SPS process. The unit cell dimensions of the α-sialon phase of
the samples listed in Table 4.5 confirm that their compositions are very close to the
oxygen-rich boundary of the α-sialon phase forming area; i.e. no matter if HP or
SPS is employed for densification, the final phase constitutions of a given
composition are the same, presumably representing thermodynamic equilibrium. A
similarly rapid phase transformation has also been observed in SPS-consolidated
rare earth-stabilised α-sialon samples with compositions ARE3512 (RE = Sm, Dy
and Y) and ANd3510 (see Table 3.1), using fast heating rates (200oC⋅min-1).
The crystalline phase content of the AY3512-10 composition is ∼50 % α- and ∼50
% β-sialon at equilibrium, as shown in Table 4.3. At ∼1400oC, 90 % of the
theoretical density is achieved, whereas the phase transformation from α-Si3N4 to
α-sialon and/or β-sialon is restricted, as manifested by the fact that the dense
compact contains 100 % un-reacted α-Si3N4. The phase transformation progresses
in a fully dense compact, however, when the temperature is increased. At ∼1650oC,
an equilibrated α/β-sialon composite is obtained, containing ∼50 % α- and ∼50 %
β-sialon. As a high heating rate 200oC⋅min-1 is used in these experiments, the phase
transformation completed within 1.25 min.
For the ALi0520 and BLi0520 compositions, the phase transformations and/or
reaction sequences that occur in dense SPS consolidated samples at temperatures
ranging from 1450 to 1750oC were investigated. The phase assemblages present, as
revealed by XRD, are given in Table 4.4. At low temperatures, 1450 and 1500oC,
the formation of α-sialon phase is favoured over β-sialon, no matter if α-Si3N4 or β-
Si3N4 is used as precursor powder. Increasing the temperature to 1600oC, the
amount of α-sialon phase formed increases and that of α-Si3N4 decreases. The
ALi0520 sample still does not contain any β-sialon phase, whereas BLi0520 is
composed of a mixture of α- and β-sialon and remaining β-Si3N4 phases. When the
temperature is increased to 1650oC, the β-sialon phase is also found in the ALi0520
sample, while BLi0520 still contains a mixture of α-and β-sialon and remaining β-
Si3N4, but with higher content of β-sialon and lower content of α-sialon and β-
Si3N4. Finally, when the temperature is increased to 1700oC for the ALi0520 and to
1750oC for the BLi0520 samples, the expected duplex α−β sialon ceramics are
1600 1650 1700 1750 18000
1600 1650 1700 1750 18003.0
Grain length Grain width
Figure 4.8 Evolution of grain geometry and fracture toughness with sintering temperature in SPS-consolidated samples, based on the AYb3512-07 composition. 4.3.3 Rapid anisotropic grain growth
The length and width of randomly selected equiaxed and elongated grains (when
present) in samples of the AYb3512, AYb3512-07 and A(Yb+Y)3512-07 com-
positions are shown in Figure 4.4, Figure 4.8 and Figure 4.9, respectively. The fully
dense compacts obtained at ∼1550oC consist of nearly equiaxed grains of sub-
micron size. Within less than 1 min, a microstructure consisting of fine equiaxed
grains transformed into a tough interlocking one consisting of well facetted,
elongated grains. This verifies that grain growth is strongly temperature-dependent
but not directly associated with the phase transformation, because the onset
temperature of grain growth for both compositions AYb3512 and A(Yb+Y)3512-07
is ~1650oC, while the transformation from α-Si3N4 to α-sialon is completed already
at 1600oC. Between 1650 and 1750oC, grains start to develop an elongated
morphology, yielding an in-situ reinforced microstructure. Obviously, above the
temperature threshold for grain growth, very fast grain growth takes place, resulting
in the formation of elongated grains with lengths ranging from a few to ten
micrometers. Similar rapid anisotropic grain growth rates have also been observed
in other RE-stabilised sialon samples as long as a transient liquid is formed or a
permanent intergranular liquid phase is present. Such rapid anisotropic growth of α-
sialon grains is hard to interpret by the static Ostwald ripening mechanism43,88,111.
Figure 4.9 The evolution of grain geometry with sintering temperature during SPS processing of the samples based on the A(Yb+Y)3512-07 composition. The inset reveals that the fracture toughness increases with the formation of elongated grains.
SEM micrographs of fracture surfaces in specimens of compositions ARE3512
(RE= Sm, Dy, Y, Yb) and ANd3510, SPS consolidated at 1830oC without holding
are shown in Figure 4.10. In these experiments a heating rate of 200oC/min was
used, and the grain growth process, once activated, progressed very rapidly, and the
resulting specimens contain elongated α-sialon grains of the same or even larger
size than those found in the Nd- and Sm-doped samples prepared by hot pressing at
1900oC for 4 hrs. Applying similar sintering parameters, in-situ reinforced
microstructures were obtained even for Y- and Yb-doped α-sialon samples, whereas
1550 1600 1650 1700 1750 1800 1850
1500 1600 1700 1800 19003,5
K 1c (
Grain length Grain width
the very same compositions hot-pressed at 1900oC for 4 hrs yielded microstructures
containing only large equiaxed grains.
Figure 4.10 SEM micrographs of fracture surfaces in samples, based on the composition ARE3512 (RE=Dy, Sm, Yb and Y) and ANd3510, after SPSing at 1830oC without holding, showing the in-situ reinforced microstructure formed in all systems investigated. The microstructure of the Y-doped sample resembles that of the Dy-doped one.
4.4 Concluding remarks
By selecting appropriate compositions and sintering parameters via the use of a new
processing concept, fully dense ceramics with tailored microstructures can be
obtained, which consist of either submicron-sized grains with equiaxed morphology
or well facetted grains with elongated morphology. This opens up new possibilities
for further materials development. It has been demonstrated that SPS is an efficient
technique to implement this new concept.
5. Sintering kinetics
The densification, phase transformation/reaction and grain growth processes are
most often observed to occur simultaneously during conventional sintering of
Si3N4-based ceramics, which implies that it is difficult to study the kinetics of each
process separately. Using SPS, however, the densification process can be
accomplished at such a low temperature that the kinetics of grain growth is retarded,
and so are the phase transformation/reactions. Furthermore, the phase
transformations/reactions can be accomplished before the grain growth process is
initiated. This therefore provides us with a unique opportunity to monitor the
kinetics of densification, phase transformation/reactions and grain growth
5.1 Densification mechanism
Typical shrinkage data recorded during densification of Si3N4-based ceramics by
SPS are given in Figures 4.4-4.7. It is difficult to interpret these data on the basis of
the classical sintering theories discussed above. The fact that full density can be
achieved with very limited involvement of phase transformation and grain growth
suggests that densification is accomplished mainly via particle rearrangement
assisted by the presence of a liquid phase. Table 5.1 summarises the main
densification characteristics of the prepared specimens. In the RE-doped sialon
system the densification started at 1200–1300oC and ended at 1480–1600oC when a
constant heating rate of 200oC⋅min-1 and a compressive stress of 50 MPa were
applied. The recorded maximum shrinkage rate is in the range of 8.5 to 13 × 10-3
sec–1. Full density was achieved when heating up to ∼1450oC, where the
transformation of α-Si3N4 to α- and/or β-sialon was of minor importance (see §
Table 5.1 Densification characteristics of specimens heated in the SPS apparatus to 1700oC.
Densification Shrinkage rate Specimens Tstart (oC) Tend (oC) Tmax (oC) εmax (s-1) AYb3512 ∼ 1300 ∼ 1550 ∼ 1460 9.0×10-3 AYb3512-07 ∼ 1250 ∼ 1500 ∼ 1451 9.4×10-3 AY3512-10 ∼ 1200 ∼ 1480 ∼ 1407 9.6×10-3 A(Y+Yb) 3512 ∼ 1250 ∼ 1600 ∼1470 8.5×10-3 A(Y+Yb) 3512-07 ∼ 1250 ∼ 1550 ∼1430 1.3×10-2 ALi1025 * ∼ 1100 ∼ 1450 ∼1420 4.8×10-3 ALi1025-17 * ∼ 1100 ∼ 1400 ∼1360 4.6×10-3
* In these cases the applied heating rate was 100oC⋅min-1.
Obviously, the rapid densification process observed in SPS differs from that in
conventional hot pressing. Figure 5.1 shows the shrinkage data recorded during SPS
processing of α-sialon based on the A(Yb+Y)3512-07 composition, when a heating
rate of 100oC⋅min-1 was used. In this particular case full density was approached
after holding at 1350oC for only 1.5 min. Three stages can be distinguished, namely
stage I) Initial particle rearrangement initiated when an oxygen-rich liquid forms;
stage II) Extensive particle rearrangement effected by grain boundary sliding; and
stage III) The final elimination of closed pores.
-200 -150 -100 -50 0 50 100 150 200
Figure 5.1 The density plotted versus time, recorded during SPS processing of a specimen based on the A(Yb+Y)3512-07 composition. The applied heating rate and uniaxial pressure are 100oC·min-1 and 50 MPa, respectively. Three densification stages are clearly revealed: I) Initial particle rearrangement; II) Extensive particle rearrangements; and III) The elimination of the closed pores.
For SPS, the most intriguing feature is the extensive second-stage particle
rearrangement that occurs dramatically fast, once activated above a critical
temperature. To determine the kinetics of this stage, Kingery’s theory was used to
simulate the relation between shrinkage and holding time. As reviewed in Chapter
1, if the densification is mainly controlled by viscous flow, the shrinkage (∆L/L0)
data should be fitted by Equation (1-1) (see §1.2.3), ∆L/L0 = k⋅ t 1+y, with the
exponent 1+y slightly larger than one. Figure 5.2a shows the linear correlation of
log (∆L/L0) with log t for the sample based on the A(Yb+Y)3512-07 composition,
when it was densified up to 90% theoretical density. The slope of these fitted lines
at 1350 and 1400oC are ∼0.59 and ∼0.17, respectively. These exponent values are
far less than 1, indicating that viscous flow is not a dominating mechanism in this
On the other hand, when the data were fitted using Kingery’s equation for a
solution-precipitation step, ∆L/L0 ∝ t 1/n, the time exponent 1/n values are ∼0.59 and
∼0.17, i.e., the measured n values are 1.7 and 5.9 at 1350oC and 1400oC,
respectively, approximating 2 and 5. This implies that a grain boundary reaction is
the rate-controlling step at 1350oC, and diffusion becomes the controlling step at
1400oC. This can be accounted for by the fact that the dissolution of AlN and Si3N4
into an early-formed oxygen-rich liquid is restricted below a certain critical
temperature (1350oC) and thus becomes the rate-controlling step. Above this
temperature, e.g. at 1400oC, the diffusion process becomes rate-controlling step
instead, because at this temperature the dissolution process takes place rapidly, and
large amount of nitrogen-containing liquid is formed. Further investigation of this
process is required in future work to determine the activation energy and reaction
constant. Anyhow, the experimental data gathered so far convincingly demonstrate
that particle rearrangement occurs very rapidly during the SPS process, whether or
not the grain boundary sliding is accompanied with a diffusion-controlled or a
reaction-controlled process in the liquid.
1.0 1.2 1.4 1.6 1.8 2.0-1.0
y:-0.69+0.17logt ρ: 0.9
Log t (Sec)
1400 oC 1350 oC
1.0 1.2 1.4 1.6 1.8 2.0 2.2-1.0
Log t (Sec)
1400 oC1300 oC1250 oC
Figure 5.2 Logarithmic shrinkage versus logarithmic time, derived from shrinkage data recorded during isothermal SPS processing of samples based on the A(Yb+Y)3512-07 (a) and ALi1025 compositions (b). In all cases, a pressure of 50 MPa and a heating rate of 100oC·min-1 were applied.
A similar densification mechanism is reasonable in the lithium-doped sialon system.
In this case, as shown in Figure 5.2b, the time exponent in the temperature range
1250–1400oC is ∼0.17, implying that the n value is 5.9. This indicates that grain-
boundary sliding accompanied by diffusion process always operates at these
temperatures, because the temperature required for dissolving Si3N4 and AlN
particles is in this case much lower.
Another fact that contributes to enhancing densification during SPS processing of
silicon nitride-based ceramics is the non-equilibrium nature of the formed liquid
phase. Due to the high heating rate applied, a concentration gradient is built up in
the liquid, so that the liquid formed close to the Si3N4 particles is rich in nitrogen, as
illustrated in Figure 5.3. When rapidly heated, the oxygen-rich part of the liquid is
brought up to a high temperature where it has very low viscosity, thus enhancing
the particle sliding under compressive stress.
Figure 5.3 A sketch map illustrating the compositional gradient in the liquid phase formed. The nitrogen concentration in the shell regions surrounding Si3N4 particles, marked with dark grey contrast, is higher than in other parts marked with light grey contrast.
5.2 Reaction sequence in fully dense ceramics
For a given overall composition, the final thermodynamic equilibrium phase
assemblies are independent of the process employed, whether conventional hot
pressing or SPS. However, the rate and the sequence of phase transformations/
reactions that will take place are strongly dependent on the precursors used, their
compositions, and the sintering parameters applied. In conventional hot pressing the
densification of Si3N4-based ceramics takes several hours, and the densification is
accompanied by phase transformations/reactions and grain growth. In the SPS
process the densification can be accomplished with very limited involvement of
phase transformations/reactions, as described in §4.3.3. Therefore, the phase
transformation/reaction sequence can be precisely followed and manipulated during
further annealing after complete densification.
For the AY3512-10 composition, the equilibrated compact contained 50 % α-sialon
and 50 % β-sialon. The temperature dependence of the phase formation that occurs
in the fully dense compact is summarised in Table 4.3, and the following reaction
sequence can be deduced:
Green body containing α-Si3N4, Al2O3, AlN, Y2O3 → Dense compact containing α-
Si3N4, AlN and an amorphous Y-Al-Si-O-N phase → Dense compact containing α-
Si3N4, α-sialon and an amorphous Y-Al-Si-O-N phase → Dense compact
containing α-Si3N4, α-sialon, β-sialon and an amorphous Y-Al-Si-O-N phase →
Dense compact containing α-sialon, β-sialon and an amorphous Y-Al-Si-O-N
In the lithium-stabilised α/β sialon sample of the composition Li0520, an α-sialon-
rich compact is initially formed, and prolonging the heat treatment yields a compact
containing equal percentages of the α- and β-sialon phases, as seen in Table 4.4.
The following schematic reaction sequence seems be valid, independent of the use
of α-Si3N4 or β-Si3N4 as starting precursor:
Green body containing Si3N4, Al2O3, AlN, Li2CO3 → Dense compact containing
Si3N4, α-sialon, AlN and an amorphous Li-Al-Si-O-N phase→ (Dense compact
containing α-sialon, and an amorphous Li-Al-Si-O-N phase) → Dense compact
containing α-sialon, β-sialon and an amorphous Li-Al-Si-O-N phase.
It appears clear that the α-sialon phase is initially formed, irrespective of whether
α-Si3N4 or β-Si3N4 is used as starting powder. Further heat treatment then induces α
to β phase transition at higher temperature.
It is worth noting that when β-Si3N4 or a coarse α-Si3N4 powder is used as starting
precursor to prepare α/β-sialon, the phase transformation from α-Si3N4 and/or β-
Si3N4 to α-sialon phase is significantly retarded. This can be interpreted in the
following manner: (i) The dissolution of coarser grains requires higher temperature;
and (ii) β-Si3N4 phase frequently contains fewer defects and less oxygen than α-
Si3N4, which is expected to retard dissolution.
The phase transformations/reactions that occur in the SPS process are controlled by
the same mechanism as in conventional hot pressing, i.e. a solution-diffusion-
reprecipitation mechanism, but it progresses much faster. This can be ascribed to
the dissolution and diffusion processes being accelerated by the pulsed electric
5.3 Grain growth mechanism
The fact that densification and phase transformation can be accomplished before
any appreciable grain growth occurs allows us to investigate the grain growth
kinetics in fully dense compacts, thus minimising the influence of porosity and
I II III
Figure 5.4. The static ripening mechanism governing grain growth during liquid-phase sintering: I) Solution; II) Diffusion; and III) Isotropic and/or anisotropic grain growth.
5.3.1 Static ripening
The static ripening mechanism has been extensively investigated and reported in the
literature43,88,111-114. It dominates the microstructure evolution of hot-pressed α-
sialon ceramics, as described in §4.1 and §4.2. Figure 5.4 illustrates schematically a
typical static ripening mechanism when sintering Si3N4-based ceramics. It clarifies
that the grain growth involves three stages: (i) Dissolution of small grains in a liquid
that is close to equilibrium with solids present; (ii) Diffusion through the liquid; and
iii) Isotropic and/or anisotropic grain growth. The characteristic features of the
static ripening process are: (i) The grain growth process is thermally activated; (ii)
The presence of a small amount liquid assists the development of elongated grain
morphology; and (iii) The grain growth occurs at a slow speed. The slow grain
boundary diffusion in the absence of a sufficient amount of liquid often masks the
diversity of interfacial reactions that determine the morphology of growing grains.
Therefore, under the static conditions it is difficult to develop an in-situ reinforced
microstructure in α-sialon ceramics with stoichiometric composition, as
exemplified in Figure 5.5.
(A) (B) (C)
Figure5.5 Microstructure development in fully dense bodies based on the A(Yb+Y)3512 composition, via different growth mechanisms: I) Static ripening; and II) Dynamic ripening. (A) Sub-micron sized equiaxied grains formed after SPSing to 1700oC without any holding time; (B) Large equiaxied grains obtained after post-heat treating of sample (A) at 1900oC for 4 hrs in a graphite furnace; and (C) Elongated grains formed after directly SPSing up to 1830oC without holding.
5.3.2 Dynamic ripening
A distinct temperature threshold for grain growth is observed in SPS-consolidated
α-sialon ceramics, above which grain growth is activated and the development of
grains with elongated morphology occurs very rapidly (within minutes), whether or
not an extra liquid is involved, as shown in §4.3. This rapid grain growth occurs in
fully dense compacts and cannot be interpreted by the static ripening mechanism.
By SPS fully dense compacts are typically obtained in the temperature range 1350–
1550oC with only a few minutes of holding, as discussed in §4.3.1 and §5.1. These
compacts consist of fine grains and usually have crystalline phase assemblies and
glass/liquid phases with compositions far from thermodynamic equilibrium.
Prolonged sintering or further annealing makes grain growth take place rapidly,
within minutes. The microstructures of AYb3512, consolidated by SPS at two
different heating rates, 200oC⋅min-1 and 40oC⋅min-1, verify that the use of fast
heating rates is essential for obtaining the required elongated grains, see Figure 5.6.
Using rapid heating rates (200oC⋅min-1) yields a microstructure with interlocking
morphology, whereas using a slow heating rate (40o C⋅min-1) does not produce
elongated grains. A heating rate of 40oC⋅min-1 is typically used in conventional hot
pressing of Si3N4-based ceramics.
We ascribe the rapid grain growth described above to an anisotropic ripening
process that takes place dynamically – abbreviated as dynamic ripening. Dynamic
ripening only occurs when the liquid phase is grossly out of thermodynamic
equilibrium with the main crystalline phase(s), i.e. is associated to a thermodynamic
state that provides a strong chemical driving force pushing the system towards
equilibrium, enhancing the dissolution of small grains and producing a momentarily
supersaturated liquid that fertilises rapid anisotropic grain growth by a diversity of
Figure 5.6 SEM photos of fractured surfaces in an α-sialon ceramic with a stoichiometric composition of AYb3512, heated to 1750oC: a) using a heating rate of 200oC·min-1; b) using a heating rate of 40oC·min-1.
5.4 Sintering kinetics Up to now it has been commonly accepted that phase transformation and reactions
leading to the formation of various sialon phases are beneficial to grain growth,
whereas the formation of rigid structure prevents further densification at the final
sintering stage115. During the SPS process, full density is accomplished with very
limited involvement of phase transformation and grain growth. This implies that
there is no obvious correlation between densification, phase
transformations/reactions and grain growth; instead, they are just three individual
temperature-dependent processes that happen to occur simultaneously in
conventional sintering processes. In SPS, the kinetics of these processes can be
more precisely determined and monitored, due to the fact that it is possible to
discern a slight difference in the onset temperatures of densification (Td), phase
transformations/reactions (Tt) and grain growth (Tg).
In general, our observations have revealed that T g≥ T t ≥ Td in silicon nitride-based
ceramics, as illustrated in Figure 5.7. These critical temperatures are adjustable by
varying the composition and processing parameters. Any adjustment of the
composition and/or processing parameters that depresses the kinetics of the
densification and/or transformation, e.g. the a and b curves are replaced by a’ and b’
in Figure 5.7, may thus make grain growth take place concurrently with densi-
fication and/or phase transformation. In order to enhance the densification process,
high temperatures are applied in conventional sintering techniques, and these
densification temperatures are often well above Tt and Tg, as determined in the SPS
a, a': Denfification rateb, b': Transformation ratec: Grain growth rate
Temperature → Figure 5.7 A schematic drawing illustrating the kinetics of three temperature-dependent processes: densification, transformation and grain growth, which often occur simultaneously in sintering of silicon nitride-based ceramics. See also text.
Below Tg the fine-grained microstructures are obtained, no matter if they consist of
equilibrium or non-equilibrium phase constituents. This type of fine-grained ceramic is
ideal for super-plastic deformation at a temperature below Tg. The fine-grained structures
can be converted to tough self-reinforced microstructures consisting of interlocking
elongated grains by post-annealing the deformed sample above Tg, as discussed above.
6. Property Evaluation
By the introduction of an extra liquid phase and/or employing the new processing
concept, α-sialon ceramics with pre-determined morphologies can be precisely and
easily developed, e.g. yielding either equiaxed or elongated grain morphologies, as
described in §4.1 to §4.3. The latter type of microstructure enhances fracture
toughness by grain bridging, crack deflection, and grain pull-out mechanisms. On
the other hand, the microstructures with fine, equiaxed grains offer a variety of
opportunities to fabricate ceramics with complicated shapes by super-plastic
The influence of the microstructure of the obtained Si3N4-based ceramics on
properties such as hardness, fracture toughness, thermal-shock resistance and super-
plastic behaviour will be elucidated in this chapter.
6.1 Mechanical properties The hardness and fracture toughness values of the prepared sialon specimens are
presented in Table 4.5, Figure 4.8 and Figure 4.9. In summary: (i) Compacts
containing elongated grains exhibit fracture toughness values in the range 5.0 to 6.5
MPa·m1/2, whereas those containing equiaxed grains have fracture toughness values
in the range 3.5 to 4.0 MPa·m1/2, verifying that compacts with interlocking micro-
structures exhibit improved fracture toughness; (ii) All α-sialon compacts have
hardness values ~20 GPa; (iii) The hardness of samples in the A(Yb+Y)3512-ZZ
series varies with the α/β content ratio from ~21 GPa to ~16 GPa, and the fracture
toughness increases concurrently from ∼3.5 to ∼6.0 MPa·m1/2 when the crystalline
assemblages present in the compact vary from monolithic α-sialon to monolithic β-
sialon via compacts containing various proportions of the α- and β-sialon phase
0 250 500 750 1000
Figure 6.1 The crack growth in percent, plotted versus the thermal-shock temperature difference for specimens based on the A(Yb+Y)3512 composition, SPS consolidated at 1700°C without holding (a), and on the A(Yb+Y)3512-07 composition, SPS consolidated at 1700°C without holding (b) and with 10 minutes holding(c).
6.2 Improved damage tolerance The cracks extensions on surfaces of the A(Yb+Y)3512 and A(Yb+Y)3512-07
compositions are plotted versus temperature difference in Figure 6.1. It is obvious
that the samples SPSed at 1700oC without holding are less resistant to thermal
shock than those prepared with a holding time of 10 min, and the curves of the
former ones resemble those reported for hot-pressed duplex α/β-sialon composites,
which are regarded as having comparatively bad thermal-shock properties116.
However, the A(Yb+Y)3512-07 samples SPSed at 1700oC with a holding time of
10 min exhibit excellent thermal-shock properties, which are quite comparable to
those of self-reinforced β-sialon ceramics containing 20 vol% glass phase, prepared
by hot pressing117.
The SEM investigation reveals that microstructures formed in the stoichiometric
A(Yb+Y)3512 composition SPSed at 1700oC without holding contains only
equiaxed grains with diameters less than ∼1 µm. When approximately 3 vol% of a
liquid phase was added to this sample, the microstructure formed at 1700oC with 10
min holding time contained elongated grains with an average diameter of 1.2 µm
and an aspect ratio of 4, distributed in a matrix of sub-micrometer-sized α-sialon
grains. This clearly confirms that the improved thermal-shock resistance of this
A(Yb+Y)3512-07 specimen can be attributed to the formation of an interlocking
microstructure. It should be noted, however, that the presence of too large acicular
grains will deteriorate the fracture strength and thus also the thermal-shock
properties, because these grains act as crack initiation sites118.
As a consequence, α-sialon ceramics that are inherently hard and contain acicular
grains of appropriate sizes, formed in situ, exhibit improved fracture toughness
values and excellent thermal-shock properties, which ought to widen their
engineering application areas, especially as wear-resistant components and cutting-
6.3 Enhanced superplasticity The rapid densification of sialon powders by the SPS process described above is
interpreted in terms of the viscosity of the liquid/glassy phase present at the grain
boundaries being reduced by the pulsed electric field. If this is correct, one expects
a similar improvement in deformation rate. We have accordingly performed
deformation tests for a variety of Si3N4-based ceramics with sub-micron sized
microstructures in the SPS apparatus and, for comparison, in a conventional hot-
pressing (HP) furnace. We have observed a radical improvement of the deformation
rate when the SPS procedure is used. Below we will present some representative
6.3.1 Lithium-stabilised monolithic α-sialon and duplex α/β-composite
The compressive strain in two lithium-stabilised sialons, of compositions ALi1025
and ALi1025-17 (see §3.2.2), has been recorded during super-plastic deformation in
the SPS apparatus and is shown in Figure 6.2. The specimens used in the
deformation experiment were compacted at 1450oC, using a holding time of 2 min
and a pressure of 50 MPa. For comparison of mechanism, the densification curves
of these compositions are also given in Figure 6.2. A maximum shrinkage rate of
4.8 × 10-3 s-1 during densification was recorded for the ALi1025 composition at
1420oC, and corresponding value for the ALi1025-17 composition at 1360oC is 4.6
× 10-3 s-1.
1000 1100 1200 1300 1400 1500 1600
Figure 6.2 The shrinkages (a0 and b0) and compressive strains (a1 and b1) recorded during densification and super-plastic deformation, plotted versus temperature. a and b represent the specimens based on the ALi1025 and ALi1025-17 compositions, respectively. Super-plastic deformation occurs surprisingly fast in the SPS apparatus as soon as
the softening temperature of the intergranular glass phases is reached. The
compressive deformation rates reached at ~1420oC and ~1380oC for the ALi1025
and ALi1025-17 compositions, respectively, are both in the range ~5.0×10-3 s-1, i.e.
comparable to the observed densification rates. This indicates that both processes
depend on the same mechanism; i.e. the low-viscosity liquid allows a rapid flow of
the sub-micron sized grains along the grain boundary under compressive stress.
The fact that no deformation occurs in the fully densified specimens at ∼1100oC –
the eutectic temperature in the Li-Si-Al-O system – indicates that it is an oxynitride
liquid/glassy phase that remains at the grain boundaries in the pre-prepared fully
densified specimens. The observed difference between the super-plastic onset
temperatures, ∼1380 and ∼1300oC for the ALi1025 and ALi1025-17 compositions
respectively, suggests that the amount of liquid is less and its viscosity presumably
higher in ALi1025 than in ALi1025-17.
Figure 6.3 SEM photos of the fracture surfaces in SPS consolidated specimens based on the ALi1025 (a) and ALi1025-17 compositions (b), and after deformation up to 1490oC for a specimen based on ALi1025 (c) and up to 1450oC for a specimen based on ALi1025-17 (d). The microstructures of these specimens are very similar before and after the
deformation, as seen in Figure 6.3. Accordingly, there is no noticeable strain
hardening, a process that has often been observed during super-plastic deformation
of silicon nitride-based ceramics by more conventional methods. We ascribe the
absence of strain hardening to the fact that the compacts used in the deformation
experiments contain non-equilibrated phase assemblages, and that the reactions
leading to thermodynamic equilibrium are retarded at the temperatures where the
compaction and deformation experiments were performed.
6.3.2 Y-/Yb-doped monophasic α-sialon and β-sialon
The two compositions A(Yb+Y)3512-07 and G20B06 (see §3.2.3) were first
consolidated to full density by the SPS process at 1500oC for 2 min and 1550oC for
4 min, respectively. Their super-plastic behaviour was then tested in the SPS
apparatus. These two dense compacts could be deformed dramatically rapidly above
1450oC and 1500oC, respectively, and strains of ∼50% were achieved within ~2
minutes, as seen in Figure 6.4a. For comparison, the very same experiment was
carried out with the HP equipment, but in this case the A(Yb+Y)3512-07 and
G20B06 specimens could not be deformed until the temperature reached 1700 and
1800oC, respectively, and then with much lower strain rates. Compressive strain
rates in the order of 10-2 s-1 can easily be achieved at T ≥ 1500oC in the SPS
apparatus. This rate is 2 orders of magnitude higher than has ever been achieved in
conventional HP deformation experiments.
1350 1400 1450 1500 1550
800 1000 1200 1400 1600 1800
0 1 2 3 4
Figure 6.4 Rapid deformation of α- and β-sialon ceramics recorded in the presence of an electric field. α and β represent the A(Yb+Y)3512-07 and G20B06 compositions, respectively. The α1 and β1 samples exhibited ultra-fine-grained microstructures, whereas α2 and β2 samples possessed tough interlocking microstructures consisting of fibrous grains. a) The obtained compressive strain data plotted versus temperature for samples deformed in an SPS apparatus and in a conventional HP furnace, respectively; b) Isothermal compressive strain data for α and β-sialon samples, recorded as functions of time at 1500oC.
The microstructures of these two sialon compacts, before and after the compressive
SPS deformation, were examined by scanning electronic microscopy (SEM). The
SPS pre-consolidated compacts, A(Yb+Y)3512-07 and G20B06, consisted of fine
equiaxed grains with average sizes of 210 and 350 nm, respectively, and both
compacts contained only very small amounts of grain-boundary glassy phase (less
than 5 vol % as estimated from SEM micrographs). The deformed samples did not
contain any elongated grains, and no grain growth was found in the G20B06
sample, whereas the average grain size in the A(Yb+Y)3512-07 sample increased
from 210 nm to 490 nm.
Isothermal compressive-strain data for the same compositions, A(Yb+Y)3512-07
and G20B06, recorded at 1500oC are plotted versus time in Figure 6.4b. The graph
brings out a strong correlation between ductility and microstructural features. The
α1 and β1 specimens, with ultra-fine equiaxed morphology, exhibit much faster
super-plastic deformation than the α2 and β2 specimens, which have tough and
interlocking microstructures. The very same α1 and β1 specimens were also
isothermally deformed in HP at 1600oC for 30 min, using a pressure of 40 MPa,
yielding compressive-strain rates of 1.4 × 10-4 s-1 and 2.0 × 10-5 s-1 for α1 and β1,
respectively. These values are two orders of magnitude lower than obtained with
SPS at 1500oC.
It should be noted that the experimental conditions are identical in the SPS and HP
deformation tests. The main difference between the two experiments is that in the
SPS apparatus the samples are exposed to a pulsed electric field. We interpret our
findings in terms of the electric field lowering the viscosity of the grain-boundary
glassy/liquid phase, thus facilitating the motion of charged species at the grain
boundary and thus yielding an increased deformation rate. The use of a pulsed
direct current (electric field) seems essential, for the application of a static electric
field may give rise to permanent charge separation in the glassy phase.
Additionally, owing to the rapid deformation in an electric field at low temperature,
the grain growth is suppressed during the deformation process. After the
compressive deformation the specimens still retain the submicron-sized equiaxed
morphology, which can easily transform to an interlocking microstructure by further
annealing/post-heating at a temperature above Tg, where dynamic ripening can take
place. Materials with this type of microstructure exhibit compressive strain rates of
the order 10-4 s-1, even in the presence of pulsed electric field. This confirms that the
formation of fine equiaxed grains is essential for super-plastic behaviour of
ceramics. In conjunction with the formation of interlocking microstructures, the
fracture toughness increases from typically below ∼3 MPa·m½ to above ∼5 MPa·m½.
Figure 6.5 A photsialon ceramic in athe SPS apparatus.
6.3.3 Near net-sh
The enhanced sup
component was d
a minor amount
in near net-shape
ograph of a component formed by super-plastic deformation of an α- graphite die at 1600oC for 2 min, in the presence of an electric field in
er-plastic deformation rates discussed above make it possible to
ts of complex shape, as exemplified in Figure 6.5. This α-sialon
eformed into its final shape at 1600oC within 2 min and contained
of grain boundary liquid phase. The deformed component is of
e, with sharp edges and excellent surface finish, indicating that
i3N4-based ceramic objects with complex shape can be prepared
These achievements demonstrate the unique possibility to achieve super-plastic
deformation of Si3N4-based ceramics containing very little glassy phase, which are
suitable for high-temperature applications. The present finding implies that cost-
effective industrial production of Si3N4-based components with complex shape is
feasible via super-plastic deformation. This concept should also be applicable to
other materials that are obtained by liquid-phase sintering.
7. Present understanding of the SPS process for enhancing the liquid phase sintering
7.1 Phenomena observed with the SPS apparatus The common phenomena so far observed during the SPS processing of Si3N4-based
ceramics may be summarised as follows: (i) Densification, phase transformation
and grain growth processes are accelerated and take place sequentially, providing
e.g. the possibility to separate grain growth from phase transformation and
densification in monitoring the kinetics; (ii) Compressive deformation progresses
much faster in the SPS apparatus than in conventional hot-pressing equipment, as
verified by the observation that the strain rate of the very same sample in the former
apparatus is two orders of magnitude larger than that in the latter; (iii) The
microstructures of SPS consolidated materials can be precisely regulated, with
better understanding and control of the sintering kinetics; and (iv) Dynamic ripening
dominates the grain growth in a rapid SPS process.
The unique features of the SPS process provide the possibility of using very fast
heating and cooling rates and very short holding times (in the order of minutes) to
obtain fully dense ceramics. In addition, the pulsed electric field used for the SPS
process may be expected to decrease the viscosity of the formed liquid phase due to
the accelerated motion of the charged species in the liquid phase. The presence of
this electric field thus seems to be another key factor in the SPS process.
7.2 Benefits of a rapid heating rate
The effect of heating rate on the microstructure of Si3N4-based ceramics is
exemplified in Figure 5.6. The use of rapid heating rates appears to be essential in
order to obtain fully dense Si3N4 ceramics with interlocking microstructures. The
major advantages of using rapid sintering rates may be summarised as following: (i)
The grain growth at the early stage of sintering is suppressed; (ii) The capillary
force between particles increases throughout the densification cycle owing to very
limited grain growth; (iii) The formation of undesirable intermediate phases is
avoided; and (iv) The non-equilibrium nature of the liquid formed contributes to the
enhancement of both densification and grain growth.
7.3 Benefits of pulsed DC heating
Pulsed DC heating has a unique effect on the sintering and the super-plastic
deformation behaviour. During the entire sintering cycle, the sample is exposed to a
pulsed electric field. Such a field exerts significant influence on the liquid-phase
sintering. The major benefits may be summarised as follows: (i) The pulsed electric
field most probably induces the process that enhances the densification rate, and
therefore it ought to be operative only in the vicinity of the grain boundaries during
the early stage of sintering; (ii) The pulsed electric field accelerates the homo-
genisation and the penetration of the liquid formed, and it therefore greatly
promotes the diffusion and mass transfer processes during the densification period;
(iii) The electric field lowers the viscosity of the grain-boundary glassy/liquid phase
via promoting the motion of charged species, which in turn promotes grain
boundary sliding and thus results in an increased densification and deformation rate.
7.4 Benefits of the use of high pressures
The possibility of applying high mechanical pressure in SPS process increases the
possibility of manufacturing hard-to-make materials, e.g. of obtaining fully dense
Si3N4-based ceramics within shorter time and at lower temperature than through a
conventional hot-pressing process. High pressures have significant influence on the
sintering process, especially in connection with liquid-phase sintering. The
following advantages of the use of high pressures can be discerned: (i) The density
of the green body is greatly increased, and thus the distance of mass transfer and
diffusion at intermediate sintering stages is reduced; (ii) The extent and rate of
particle rearrangement is increased; (iii) The homogenisation and penetration of the
liquid phase along grain boundaries may be expected to be enhanced.
7.4 Future work
Due to the inherent time limitation of a PhD thesis, I have not been able to explore
the possibility of preparing truly nano-sized silicon nitride-based ceramics by SPS,
or to consolidate other ceramics by applying this novel processing concept. I should
therefore like to work along the following lines in the near future:
i) Preparing nano-structured silicon nitride ceramics by SPSing truly nano-
sized precursor powders;
ii) Manufacturing ceramic components of complex shape by super-plastic
deformation of the fully dense nano-structured ceramics obtained;
iii) Reaching better understanding of the enhanced sintering kinetics;
iv) Fabricating laminated composites consisting of nano-/micro-sized Si3N4
and SiC layers with tailored microstructures by manipulating the grain
v) Enlarging the application field of SPS, e.g. to sintering new materials
that may be impossible to achieve by conventional sintering methods.
Some of this work can be regarded as a natural continuation of my PhD work,
others parts will be more explorative.
Monophasic α-sialons with both stoichiometric and non-stoichiometric overall
starting compositions have been consolidated by the SPS process and subsequently
investigated with respect to their microstructures and mechanical properties. For
comparison, appropriate experiments have also been performed by means of
conventional hot pressing (HP). Although it is very difficult to achieve elongated
grain morphology in monophasic α sialon with stoichiometric composition by
means of the HP process, it is possible to obtain an interlocking microstructure,
consisting of elongated grains, in the presence of extra liquid introduced.
A liquid phase, thermodynamically compatible with α-sialon, was introduced by a
new method, i.e. slightly increasing the O/N ratio of an already oxygen-rich α-
sialon composition, while keeping the cation ratios of the sialon phase, RExSi12-
(3x+n)Al3x+nOnN16-n, constant. Reinforced microstructures were developed in situ in
Y-, Yb-, and (Y+Yb)-stabilised α-sialon ceramics containing ~3 vol% liquid phase,
by means of a HP process at 1800oC for 4 hrs.
The SPS process is a promising technique that allows a better understanding of
sintering kinetics and therefore makes it possible to obtain Si3N4-based ceramics
with tailored microstructures, consisting of either fine, equiaxed or elongated grain
morphology via manipulation of the sintering kinetics.
Densification, phase transformation/reactions and grain growth are three individual
temperature-dependent processes that can be studied separately in most sialon
systems by applying the SPS process, because the onset temperatures of
densification (Td), phase transformations/reactions (Tt) and grain growth (Tg) are
sufficiently different. In general, our observations reveal Tg ≥ Tt ≥ Td in silicon
nitride-based ceramics. These critical temperatures are adjustable by changing the
composition and by selecting appropriate processing parameters.
Fully dense Si3N4-based ceramics can be produced in the SPS process merely by
enhanced particle rearrangement via grain boundary sliding accompanied by either
diffusion- or reaction-controlled process in the liquid, without, or with very limited
grain growth. The rapid densification is ascribed to the retention of a fine particle
size throughout the densification cycle, and to the creation of a non-equilibrium
liquid phase by rapid heating.
Rapid grain growth after complete densification and phase transformation is
accomplished by heat treatment at temperatures above Tg and by the use of high
heating rates; this growth is driven by the dynamic ripening mechanism. This
mechanism acts only when the liquid phase is grossly out of thermodynamic
equilibrium with the main crystalline phase(s) present. As the entire system
approaches its thermodynamic equilibrium state, the grain growth mechanism
changes from dynamic to static ripening.
The interlocking microstructure is responsible for improved mechanical properties,
e.g. compacts containing elongated grains exhibiting fracture toughness values in a
range from 5 to 6.5 MPa·m1/2, whereas those containing equiaxed grains exhibited
corresponding values in the range from 3.5 to 4.0 MPa·m1/2. The refined
interlocking microstructure of monophasic α-sialon ceramics exhibits excellent
thermal-shock properties, quite comparable to those of the best hot-pressed, self-
reinforced β-sialon ceramics containing 20 vol% glass phase.
The possibility of producing ceramics with fine, equiaxed grain morphologies is a
key factor in connection with the tailoring the super-plastic properties of the
materials. Thus Si3N4-based ceramics with fine equi-axed grain morphologies
exhibit a formidable improvement of super-plastic behaviour in the presence of an
electric field, whether or not a monophasic α- and β- sialon or a duplex α/β- sialon
composite is involved. A compressive strain rate of the order 10-2 s-1 is observed at
temperatures exceeding 1500oC, which is two orders of magnitude higher than that
ever achieved by the HP process, confirming that the super-plastic deformation
takes place very rapidly in the SPS process. The enhanced ductility is accounted for
by enhanced grain boundary sliding in the presence of a pulsed electric field, which
in turn decreases viscosity of the glassy/liquid phase and increases the diffusivity
within this phase. The rapid super-plastic deformation observed in this work opens
up possibilities of making ceramic components with complicated shapes, e.g.
production of near net-shaped ceramic cutting tool blanks with special geometries
seems to be feasible.
Finally, I wish to express my sincere thanks to all the people who, in different ways,
have supported me and helped me to complete this thesis, and who have made my
stay in Sweden comfortable and enjoyable. Especially, I would like to thank the
First of all, I wish to express my deepest gratitude to Doc Zhijian Shen, my
supervisor, who introduced me to the field of Si3N4 ceramics and who has guided
my doctoral studies all the way. I would like to thank you for supporting and
encouraging me throughout these years. Your incredible enthusiasm and optimistic
dedication to science has impressed me deeply. I am especially grateful for your
great ability, not only to share your academic knowledge but also to help organise
my research, which has contributed to making my thesis and publications
comprehensive. Your door has always been open, and I have immeasurably
treasured your advice and guidance, both in the scientific field and in daily life.
Without your help and support, it would have been impossible for me to complete
this thesis. Many thanks also to your family for the kindness and generosity that
made the first year of my stay in Sweden much easier. The moments when you let
me share delicious food and nice barbecues are highly appreciated and
I also thank Professor Mats Nygren, my co-supervisor, for inviting me to Sweden
and accepting me as PhD student, for all the support and help from you whenever
needed, and for creating a most stimulating working atmosphere of scientific
freedom. I am also grateful for your great interest in my work and for taking time to
correct my papers and my thesis.
Prof Sven Lidin, for creating a stimulating and pleasant scientific environment, and
of course, for your interest in my work and thesis and for always being helpful.
Prof Osamu Terasaki, for your interest and concerns in my thesis, and also for your
comments and encouragement.
Dr Kjell Jansson, for teaching me to use the scanning electronic microscope (SEM)
and for always being available for endless questions about that technique.
Dr Pernilla Magnusson: you are so sweet and considerate, thank you so much for
sharing your office with me, for nice coffee breaks, for your considerateness and
help, and of course, for teaching me how to perform thermal-shock measurements
and for our joint publication of one paper.
Mr Lars Göthe, for always cheerfully accepting my samples, for recording and
developing innumerable Guinier–Hägg films, and also for finding my mislaid
Mrs Jaroslava Östberg, for you never-ending helpfulness with my SEM samples,
and for valuable discussions on my visit to Prague, and of course for extensive help
and for coaching my Swedish.
Per-Erik Persson and Rolf Eriksson, for being available and helpful in solving
computer problems; you are real good virus-killers!
Mr Mats Carlsson, for valuable tips and discussions about my thesis; also for
lending me the first Swedish children’s book I ever read, for coaching my Swedish,
and for all your wonderful help and coffee breaks.
Ms Hillevi Isaksson, for always being helpful with literature searches and for
installing the search-engine program, and also for nice conversations and laughs
during lunches and coffee breaks.
Dr Zhe Zhao, for all valuable discussions and help, both in and out of the lab.
Special thanks to you for solving tough computer problems when I got my first new
Mss Eva Pettersson and Ann-Britt Rönell – you are so nice and warm-hearted;
thank you so much for all your help. I wish to thank Ann-Britt especially for
considerateness and understanding; and of course, your help and advice on
organising my disputation party are highly appreciated. You are so helpful
whenever I have a problem.
Doc Sven Westman for language revision of my articles and thesis.
Everyone at KÖL–Thank you! Prof Ingrid Bryntse, Dr Monica Lundberg, Mss
Yvonne Djurberg, Åsa Borin, Maria Petersson, Mr Arne Sjödin & Mr Victor Bravo
Vicuna. Many thanks to Ingrid, my ex-roommate, for sharing your office with me
and for all concerning and help specially during my first year in Sweden. Your help
and kindness are highly appreciated.
Dr Martin Valldor is greatly thanked for supervising my project “Metal Substitution
in the spin-glass YBaCo4O7” when I attended the Materials chemistry course, and
for introducing me into a different world; I am very impressed by your enthusiasm
for new structures and crystals.
Ms Emma Firman, whom I worked with when I was a teaching assistant for the first
time, for being always kind and helpful. You are so good at pedagogy and teaching.
Your help and encouragement are highly appreciated and unforgettable.
Dr Lars-Johan Norrby, for helpful advice and discussions during my teaching
experience as a laboratory assistant, and of course also for your understanding and
considerateness. Thank you!
Dr Annika Pohl, for those long and wonderful coffee breaks and summer excursions
together, and for being a good friend. You are so sweet and considerate. I miss you
so much since you moved to Uppsala University.
Mr Andreas Flemström, for being such a wonderful and constantly cheerful friend. I
would like to thank you for showing me Stockholm, guiding me to nice restaurants,
and teaching me how to use the microscope. Of course, thank you also for all joyful
coffee break and jokes and laughs. “Tack så mycket! Min första svenska lärare, men
tyvärr, jag är fortforande jätte dålig på uttalet av “r”. Tack för träning ändå!”
Mr Henrik Rundgren, you are so open, nice and easy to talk with. “Tack så jätte
mycket för otroligt goda kakor och buller. Framför allt för de goda tiderna när vi har
fikat och skrattat åt! ”
Many thanks also go to my ex- and present-roommates, Dr Göran Nilsson, Ms
Hanna Lind and Mr Richard Becker for spending a number of years with me,
always willing to help and sharing a problem and for creating a stimulating and
pleasant atmosphere to work in. Thank you so much!
All Chinese colleagues and friends within the department: Doc Xiaodong, Dr Ye
Zhou, Dr Tuping, Dr Yiqiu, Zheng Weng, Dr Yaoquan, Joan Liu, Suying, Juanfang,
Hong Zhang, Dr Zhen Liu, Yanbing, Drs Weikang & Yafeng – you all are so warm-
hearted and helpful, both in and out of the lab. Your help and advice are treasured.
Special thanks to Dr Yezhou for being my witness in obtaining an ID card, and for
all the help I desperately needed when newly arrived in Sweden.
To friends outside the lab
All my friends out of the lab are of great importance to me. All of you enrich my
life and make it more colourful and joyful, with parties, playing, games, fishing and
trips together, big as well as small events. All those wonderful times are
unforgettable and highly appreciated. I wish to thank all of you as much as I can. I
cherish your friendship and your considerateness. I wish to thank the following
Thorvald Staaf, min ex-korridor-kompis, du är den underbaraste vän som jag och
Liqiu någonsin har haft. Tack för allt stöd och all uppmuntran. Utan din hjälp skulle
jag inte kunna tala så ”bra” svenska. Jag vill även tacka dig för lördagsfesterna,
båtutflykterna, onsdagsfilmerna och de många vykort som du skickat. Javisst, jag
vill jättegärna tacka dig för din påminnelse: ”Jobba inte så hårt! Njut av livet!”
Detta är jätteviktigt! Tack!
Ett stort tack går också till min franske vän Oliver, mina tyska vänner Thomas,
Stephan och min italianske vän Fabio, för alla våra fester och vår glädje
Many thanks go to Wujiang, HuangZhen, Jiawei, Sunwei Zhu and Inger Jiang, for
all the fun we have had together, for all kinds of trips and excursions together, and
also for those long discussions about making food, playing badminton and planning
parties (you know?). I wish those wonderful, good times will remain with me
Wanjue and Lixin, for all weekend-shopping excursions, help, encouragement and
consideration; and also for the summer activities in “our common garden”. Special
thanks to lovely Diandian, for your “lördagsgodis” and the gladness you bring to
me. I miss you so much since you left.
I wish to express great gratitude to Yaodong, Chen Yan, Huang Fang, Lingwan
Wang for all joy, encouragement and help. Special thanks to Yaodong, for your
guidance in planting flowers and also for sharing DVD films. Without you guys, my
life would have been monotonous and boring.
Roger Ericsson, Kaihong and Kaimei, my ski coaches: thank you so much for your
instruction, patience, and encouragement, for skiing and for friendship. I had such a
fantastic a ski-trip; a wonderful experience that I will never forget. I already long
for the next trip with you.
I wish to thank Liuwei, who is the “leader” of MBA (you know) and always
positive and glad, and all MBA members during my first year in Sweden. All our
activities together relieved my homesick feelings and made my life colourful and
Here I would like to thank my closest friend Xinchun Tan from high school in
China, for always helping me to remember things in China, and for helping and
caring for my family.
…… to everyone who has contributed to the thesis in any way, even if you are
not mentioned, you are definitely not forgotten!
To my family
Thanks you so much, Mama; you are always so strong and brave, struggling with all
difficult situations by yourself so that I can concentrate on my work and smoothly
finish my studies abroad. Your endless support and understanding are my driving
force. Finally, your daughter has grown up – she can handle anything. Believe in
her! Please enjoy your life and relax. I owe you so much, Mama!
I also want thank my brother and my sister-in-law for taking care of mother and
keeping her company when I am abroad. Of course, I would also like to thank my
favourite nephew for all his laughs and the happiness he brings to our family.
Last but not least, I would like to express my deepest gratitude to my life partner,
Liqiu, who is the light of my life. Thank you so much for ten-year journey together,
for all tears and happiness we have had together, and also for your endless support,
encouragement and love. With you, life will never be boring.
1. Jack, K. H. Prospects for nitrogen ceramics in engine applications.
International Symposium on Ceramic Materials and Components for
Engines -- 5th, Shanghai, May 29-June 1, 1994, 32-8 (1995).
2. Jack, K. H. Nitrogen ceramics for engine applications. Materials Science
Forum 325-326, 255-262 (2000).
3. Lange, F. F. Strong, high-temperature ceramics. Report, Westinghouse Res.
Lab, Pittsburgh PA USA. FIELD URL, 78 pp. (1974).
4. Lange, F. F. High-temperature strength behavior of hot-pressed silicon-
nitride. Evidence for subcritical crack growth. Journal of the American
Ceramic Society 57, 84-7 (1974).
5. Lange, F. F. Fracture toughness of silicon nitride (Si3N4) as a function of the
initial α-phase content. Journal of the American Ceramic Society 62, 428-30
6. Lange, F. F. High temperature deformation and fracture phenomena of
polyphase silicon nitride materials. NATO ASI Series, Series E: Applied
Sciences 65, 467-90 (1983).
7. Lewis, M. H. Plasticity and fracture mechanisms in ceramic alloys based on
b-silicon nitride (Si3N4). Micromech. Plast. Fract. [Rev. Pap. Symp. Honour
Dr. J. W. Martin], 181-224 (1983).
8. Lewis, M. H. Sialons and silicon nitrides; microstructural design and
performance. Materials Research Society Symposium Proceedings 287, 159-
9. Lewis, M. H. Microstructural design of Si3N4 and Sialon ceramics in relation
to combined mechanical and environmental behavior. NATO ASI Series,
Series E: Applied Sciences 267, 425-39 (1994).
10. Lewis, M. H. Ceramic matrix composites. NATO ASI Series, Series 3: High
Technology 15, 599-624 (1996).
11. Lewis, M. H. Sialons and silicon nitrides as high temperature engineering
materials; retrospect and prospect. NATO ASI Series, Series 3: High
Technology 15, 545-566 (1996).
12. Hardie, D. & Jack, K. H. Crystal structures of silicon nitride. Nature
(London, United Kingdom) 180, 332-3 (1957).
13. Zerr, A. et al. Synthesis of cubic silicon nitride. Nature (London, United
Kingdom) 400, 340-342 (1999).
14. Sekine, T. Shock synthesis of cubic silicon nitride. Journal of the American
Ceramic Society 85, 113-116 (2002).
15. Hampshire, S., Park, H. K., Thompson, D. P. & Jack, K. H. α'-Sialon
ceramics. Nature (London, United Kingdom) 274, 880-2 (1978).
16. Mitomo, M., Kuramoto, N. & Suzuki, H. The formation of single phase β-
sialon. Proc. Ing. Symp. Factors Densification Sintering Oxide Non-Oxide
Ceram., 463-7 (1979).
17. Mitomo, M. & Kuramoto, N. The formation of β-sialon in the system
silicon-aluminum-oxygen-nitrogen (Si3N4-SiO2-AlN). Yogyo Kyokaishi 87,
18. Nordberg, L. O. & Ekström, T. Hot-pressed MoSi2-particulate-reinforced α-
SiAlON composites. Journal of the American Ceramic Society 78, 797-800
19. Shen, Z. J., Nordberg, L. O., Nygren, M. & Ekström, T. α-Sialon grains with
high aspect ratio-Utopia or reality? NATO ASI Series, Series 3: High
Technology 25, 169-178 (1997).
20. Chen, I. W. & Rosenflanz, A. A tough SiALON ceramic based on α-Si3N4
with a whisker-like microstructure. Nature (London) 389, 701-704 (1997).
21. Nordberg, L.-O., Shen, Z., Nygren, M. & Ekström, T. On the extension of
the α-Sialon solid solution range and anisotropic grain growth in Sm-doped
α-Sialon ceramics. Journal of the European Ceramic Society 17, 575-580
22. German, R. M. Liqiud phase sintering. Plenum press, New York and
23. Kingery, W. D. Densification during sintering in the presence of a liquid
phase. I. Theory. Journal of Applied Physics 30, 301-6 (1959).
24. Lifshitz, I. M. & Slyozov, V. V., The Kinetics of Precipitation from
Supersaturated Solid Solutions. Journal of Physical Chemistry Solids 19, 35-
25. Wagner, C. Theory of Precipitate Change by Redissolution. Z. Electrochem.
26. Ardell, A. J. Effect of volume fraction on particle coarsening. Theoretical
considerations. Acta Metallurgica, 20 61-71 (1971).
27. Becher, P. F., Hwang, S. L., Lin, H. T. & Tiegs, T. N. Microstructural
contributions to the fracture resistance of silicon nitride ceramics. NATO ASI
Series, Series E: Applied Sciences 276, 87-100 (1994).
28. Lewis, M. H. Crystallization of grain boundary phases in silicon nitride and
Sialon ceramics. NATO ASI Series, Series E: Applied Sciences 276, 217-31
29. Hwang, S. L. & Chen, I. W., Reaction hot pressing of α'- and β'-SiAlON
ceramics. Journal of the American Ceramic Society 77, 165-71 (1994).
30. Iskoe, J. L. & Lange, F. F. Development of microstructure and mechanical
properties during hot pressing of silicon nitride (Si3Ni4). Ceram. Microstruct.
Proc. Int. Mater. Symp. 6th, 669-78 (1977).
31. Jack, K. H., The significance of structure and phase equilibriums in the
development of silicon nitride and Sialon ceramics. Science of Ceramics 11,
32. Bowen, L. J., Carruthers, T. G. & Brook, R. J. Hot-pressing of Si3N4 with
Y2O3 and Li2O as additives. Journal of the American Ceramic Society 61,
33. Bowen, L. J., Weston, R. J., Carruthers, T. G. & Brook, R. J. Hot-pressing
and the α−β phase transformation in silicon nitride. Journal of Materials
Science 13, 341-351 (1978).
34. Lee, D.-D., Kang, S.-J. L. & Yoon, D. N. Mechanism of grain growth and
α−β' transformation during liqiud-phase sintering of β'-sialon. Journal of the
American Ceramic Society 71, 803-806 (1988).
35. Hideyuki, E., Hirotsuru, H. & Mitomo, M. Microstructural development
during phase transforamtion of silicon nitride ceramics. Journal of the
Ceramic Society, Japan 106, 488-493 (1998).
36. Shimada, M., Tanaka, A., Yamada, T. & Koizumi, M. Densification and
phase transformation of silicon nitride by high-pressing sintering. Mater. Sci.
Monogr. 16 (Ceram. Powder), 871-879 (1983).
37. Hirotsuru, H., Mitomo, M. & Nishimura, T. Relation between grain growth
and phase transformation of silicon nitride. Journal of the Ceramic Society,
Japan 103 (1995).
38. Hirao, K., Nagaoka, T., Brito, M. E. & Kanzaki, S. Microstructural control of
silicon nitride by seeding with rodlike β-silicon nitride particles. Journal of
the American Ceramic Society 77, 1857-62 (1994).
39. Mitomo, M. in 6th International Symposium on Ceramic Materials and
Components for Engines (Japan Fine Ceramics Association), (1997).
40. Park, D. S., Lee, S.-Y., Kim, H.-D., Yoo, B.-J. & Kim, B.-A. Extra large
grains in the silicon nitride ceramics doped with yttria and hafnia. Journal of
the American Ceramic Society 81, 1876-80 (1998).
41. Zhang, C., Komeya, K., Tatami, J. & Meguro, T. Inhomogeneous grain
growth and elongation of Dy-α sialon ceramics at temperature above 1800 oC. Journal of the European Ceramic Society 20, 939-944 (2000).
42. Emoto, H. & Mitomo, M. Control and characterization of abnormally grown
grains in silicon nitride ceramics. Journal of the European Ceramic Society
17, 797-804 (1997).
43. Kitayama, M., Hirao, K., Toriyama, M. & Kanzaki, S. Modeling and
simulation of grain growth in Si3N4 I. Anisotropic Ostwald ripening. Acta
Materialia, 46 6541-6550 (1998).
44. Lewis, M. H., Bhatti, A. R., Lumby, R. J. & North, B. The microstructure of
sintered silicon-aluminum-oxygen-nitrogen ceramics. Journal of Materials
Science 15, 103-13 (1980).
45. Hampshire, S. & Jack, K. H. Densification and transformation mechanisms
in nitrogen ceramics. NATO ASI Series, Series E: Applied Sciences 65, 225-
46. Drew, R. A. L., Hampshire, S. & Jack, K. H. The preparation and properties
of oxynitride glasses. NATO ASI Series, Series E: Applied Sciences 65, 323-
47. Bowen, L. J., Carruthers, T. G. & Brook, R. J. Hot-pressing of silicon nitride
with yttrium oxide and lithium oxide as additives. Journal of the American
Ceramic Society 61, 335-9 (1978).
48. Messier, D. R., Riley, F. L. & Brook, R. J. The α/β silicon nitride phase
transformation. Journal of Materials Science 13, 1199-205 (1978).
49. Bowen, L. J., Weston, R. J., Carruthers, T. G. & Brook, R. J. Mechanisms of
densification during the pressure sintering of α-silicon nitride. Adv. Ceram.
Process. Proc. Int. Meet. Mod. Ceram. Technol. 3rd, 162-5 (1978).
50. Brook, R. J., Carruthers, T. G., Bowen, L. J. & Weston, R. J. Mass transport
in the hot pressing of α-silicon nitride. NATO Advanced Study Institutes
Series, Series E: Applied Sciences E23, 383-90 (1977).
51. Bowen, L. J., Weston, R. J., Carruthers, T. G. & Brook, R. J. Hot-pressing
and the α−β phase transformation in silicon nitride. Journal of Materials
Science 13, 341-50 (1978).
52. Hampshire, S. & Jack, K. H. The kinetics of densification and phase
transformation of nitrogen ceramics. Proceedings of the British Ceramic
Society 31, 37-49 (1981).
53. Jack, K. H. The role of additives in the densification of nitrogen ceramics.
Report. Univ. Newcastle upon Tyne, Newcastle upon Tyne, UK. FIELD
URL. 123 pp. (1977).
54. Rahaman, M. N., Riley, F. L. & Brook, R. J. Reaction sintering and the a-
silicon nitride (Si3N4)/β'-sialon transformation for compositions in the
system silicon-aluminum-oxygen-nitrogen. Journal of Materials Science 16,
55. Inoue, K. (US Patent NO. 3 241 956).
56. Mishra, R. S., Risbud, S. H. & Mukherjee, A. K. Influence of initial crystal
structure and electrical pulsing on densification of nanocrystalline alumina
powder. Journal of Materials Research 13, 86-89 (1998).
57. Yoshimura, M., Ohji, T., Sando, M. & Nihara, K. Rapid rate sintering of
nano-grained ZrO2-based composites using pulse electric current sintering
method. Journal of Materials Science Letters 17, 1389-1391 (1998).
58. Murayama, N. What can we do by pulsed electric current sintering?
Seramikkusu 32, 445-449 (1997).
59. Zhou, Y., Hirao, K., Toriyama, M. & Tanaka, H. Very rapid densification of
nanometer silicon carbide powder by pulse electric current sintering. Journal
of the American Ceramic Society 83, 654-656 (2000).
60. Mishra, R. S. & Mukherjee, A. K. Electric pulse assisted rapid consolidation
of ultrafine grained alumina matrix composites. Materials Science &
Engineering, A: Structural Materials: Properties, Microstructure and
Processing A287, 178-182 (2000).
61. Tokita, M. Trends in advanced spark plasma sintering systems and
technology. Functionally gradient materials and unique synthetic processing
methods from next generation of powder technology. Funtai Kogaku Kaishi,
30 790-804 (1993).
62. Tokita, M. Development of third-generation spark-plasma-sintering (SPS)
systems. Advanced production process for fine ceramics and functionally
gradient materials. Nyu Seramikkusu, 7 63-74 (1994).
63. Tokita, M. Present situation and future prospects of spark plasma sintering
(SPS) system. Shinsozai, 7 19-28 (1996).
64. Tokita, M. Current status of spark plasma sintering. Sokeizai 41, 8-13 (2000).
65. Tokita, M. Spark plasma sintering apparatus. Nanoryushi no Seizo-Hyoka-
Oyo-Kiki no Saishin Gijutsu, 146-153 (2002).
66. Hirota, K., Nakane, S., Yoshinaka, M. & Yamaguchi, O. Spark Plasma
Sintering (SPS) of several intermetallic compounds prepared by Self-
propagating High-temperature Synthesis (SHS). International Journal of
Self-Propagating High-Temperature Synthesis 10, 345-358 (2002).
67. Liu, Q., Jiang, D., Huang, Z., Shen, Z. & Nygren, M. Improved densification
of Al2O3 and SiC based ceramic composites by spark plasma sintering.
Ceramic Transactions124, 127-137 (2001).
68. Mamedov, V. A. Spark plasma sintering (SPS) as advanced powder
metallurgy sintering method. Powder Metallurgy Progress (Kosice,
Slovakia) 2, 32-43 (2002).
69. Noguchi, T. Powder processing of thermoelectric materials--focusing on
SiGe with new sintering technique. International Conference on
Thermoelectrics 16th, 207-214 (1997).
70. Okutani, T. & Nakata, Y. Preparation of SiC-Si composites by plasma
sintering. Nyu Seramikkusu 7, 33-7 (1994).
71. Shen, Z. & Nygren, M. Implications of kinetically promoted formation of
metastable α-Sialon phases. Journal of the European Ceramic Society 21,
72. Tamari, N. Preparation of whisker reinforced zirconia by spark plasma
sintering. Nyu Seramikkusu 7, 43-6 (1994).
73. Zhang, J.-X. et al. Preparation of titanium nitride/alumina laminate
composites. Journal of the American Ceramic Society 85, 1133-1138 (2002).
74. Yamamoto, S., Oki, N., Kurisu, H. & Matsuura, M. Novel preparation
method of ultra-thin ferrite platelets. Journal of the Society of Inorganic
Materials, Japan 10, 115-121 (2003).
75. Gao, L., Shen, Z., Miyamoto, H. & Nygren, M. Superfast densification of
oxide/oxide ceramic composites. Journal of the American Ceramic Society
82, 1061-1063 (1999).
76. Shen, Z. & Nygren, M. Super-fast densification of bioactive and structural
ceramics and composites. Ceramic Transactions 128, 15-24 (2001).
77. Shen, Z. & Nygren, M. Kinetic aspects of superfast consolidation of silicon
nitride based ceramics by spark plasma sintering. Journal of Materials
Chemistry 11, 204-207 (2001).
78. Shen, Z. & Nygren, M. Laminated and functionally graded materials
prepared by spark plasma sintering. Key Engineering Materials 206-213,
79. Zhao, Z., Johnsson, M. & Shen, Z. Microstructure and mechanical properties
of titanium carbonitride whisker reinforced β-Sialon matrix composites.
Materials Research Bulletin 37, 1175-1187 (2002).
80. Nygren, M. & Shen, Z. On the preparation of bio-, nano- and structural
ceramics and composites by spark plasma sintering. Solid State Sciences 5
81. Shen, Z. & Nygren, M. Non-equilibrium processing of ceramics. Key
Engineering Materials 247, 79-82 (2003).
82. Shen, Z. & Nygren, M. Tailoring the microstructures of SiAlON ceramics by
manipulating the kinetics. Key Engineering Materials 237, 149-156 (2003).
83. Shen, Z., Johnsson, M. & Nygren, M. TiN/Al2O3 composites and graded
laminates thereof consolidated by spark plasma sintering. Journal of the
European Ceramic Society 23, 1061-1068 (2003).
84. Shen, Z. & Nygren, M. On the extension of the α-Sialon phase area in
yttrium and rare-earth doped systems. Journal of the European Ceramic
Society 17, 1639-1645 (1997).
85. Ekström, T. Sialon composite ceramics. Key Engineering Materials 89-91,
86. Chen, I. W., Shuba, R. A. & Zenotchkine, M. Y. Development of tough α-
Sialon. Key Engineering Materials 237, 65-78 (2003).
87. Hoffmann, M. J., Schneider, G. A. & Petzow, G. The potential of silicon
nitride for thermal shock applications. NATO ASI Series, Series E: Applied
Sciences 241, 49-58 (1993).
88. Petzow, G. & Hoffmann, M. J. Grain growth studies in silicon nitride
ceramics. Materials Science Forum, 113-115 91-102 (1993).
89. Andersson, T. & Rowcliffe, D. J. Indentation thermal shock test for
ceramics. Journal of the American Ceramic Society 79, 1509-1514 (1996).
90. Andersson, T. & Rowcliffe, D. J. Thermal cycling of indented ceramic
materials. Journal of the European Ceramic Society 18, 2065-2071 (1998).
91. Hamilton, C. H. & Paton, N. E. Superplasticity and Superplastic
deformation. Warrendale PA: Metallugical Society, (1988).
92. Wakai, F., Sakaguchi, S. & Matsuno, Y. Superplasticity of yttria-stabilized
tetragonal zirconia polycrystals. Advanced Ceramic Materials 1, 259-63
93. Wakai, F., Kato, H., Sakaguchi, S. & Murayama, N. Compressive
deformation of yttrium oxide-stabilized zirconium oxide/aluminum oxide
composite. Yogyo Kyokaishi 94, 1017-20 (1986).
94. Kondo, Y. & Wakai, F. Superplastic ceramics. Sokeizai 27, 13-19 (1986).
95. Chen, I. W. & Xue, L. A. Development of superplastic structural ceramics.
Journal of the American Ceramic Society 73, 2585-609 (1990).
96. Wakai, F., Sakaguchi, S. & Kanzaki, S. Process for superplastic molding of
ceramic material in Ger. Offen. Agency of Industrial Sciences and Technology,
Japan; Japan, Ministry of International Trade and Industry, 12 pp. (1986).
97. Wakai, F. et al. A superplastic covalent crystal composite. Nature (London,
United Kingdom) 344, 421-3 (1990).
98. Kim, B. N., Hiraga, K., Morita, K. & Sakka, Y. A high-strain-rate
superplastic ceramic. Nature (London, United Kingdom) 413, 288-291
99. Wang, J. G. & Raj, R. Mechanism of superplastic flow in a fine-grained
ceramic containing some liquid phase. Journal of the American Ceramic
Society 67, 399-409 (1984).
100. Wakai, F., Kondo, N. & Shinoda, Y. Ceramics superplasticity. Current
Opinion in Solid State & Materials Science 4, 461-465 (1999).
101. Mitomo, M., Hirotsuru, H., Suematsu, H. & Nishimura, T. Fine-grained
silicon nitride ceramics prepared from β-powder. Journal of the American
Ceramic Society 78, 211-14 (1995).
102. Rosenflanz, A. & Chen, I. W. "Classical" superplasticity of Sialon ceramics.
Journal of the American Ceramic Society 80, 341-1352 (1997).
103. Kondo, N., Ohji, T. & Wakai, F. Strengthening and toughening of silicon
nitride by superplastic deformation. Journal of the American Ceramic
Society 81, 713-716 (1998).
104. Hwang, S.-L. & Chen, I. W. Superplastic forming of Sialon ceramics.
Journal of the American Ceramic Society 77, 2575-85 (1994).
105. P.-E. Werner. A Fortran program for least-squares refinement of crystal
structure cell dimensions. Arkiv för kemi 31, 513-516 (1969).
106. Shen, Z., Ekström, T. & Nygren, M. Homogeneity region and thermal
stability of neodymium-doped α-Sialon ceramics. Journal of the American
Ceramic Society 79, 721-32 (1996).
107. Shen, Z., Ekström, T. & Nygren, M. Ytterbium-stabilized α-Sialon ceramics.
Journal of Physics D: Applied Physics 29, 893-904 (1996).
108. Ekström, T., Käll, P.-O., Nygren, M. & Olsson, P. O. Dense single-phase β-
sialon ceramics by glass-encapsulated hot isostatic pressing. Journal of
Material Science 24, 1853-1861 (1989).
109. Anstis, G. R., Chantikul, P., Lawn, B. R. & Marshall, D. B. A critical
evaluation of indentation techniques for measuring fracture toughness: I,
Direct crack measurements. Journal of the American Ceramic Society 64,
110. Evans, A. G. & Charles, E. A. Fracture toughness determinations by
Indentation. Journal of the American Ceramic Society 59, 371-372 (1976).
111. Pezzotti, G., Kleebe, H.-J., Nishida, T. & Ziegler, G. Growth isotherms of
liquid-phase sintered silicon nitride. Journal of the Ceramic Society, Japan
105, 638-640 (1997).
112. Kitayama, M., Hirao, K., Toriyama, M. & Kanzaki, S. Anisotropic Ostwald
ripening in β-Si3N4 with different lanthanide additives. Ceramic
Transactions 83, 517-524 (1998).
113. Kraemer, M., Hoffmann, M. J. & Petzow, G. Grain growth studies of silicon
nitride dispersed in an oxynitride glass. Journal of the American Ceramic
Society 76, 2778-84 (1993).
114. Tikare, V. Numerical simulation of grain growth in liquid phase sintered
materials (ceramics, silicon nitride, Ostwald ripening). Thesis. Case Western
Reserve Univ., Cleveland ,OH, USA. FIELD URL: 203 pp. (1996).
115. Petzow, G. & Herrmann, M. Silicon nitride ceramics. Structure and
Bonding(Berlin, Germany), 102(High Performance Non-Oxide Ceramics II),
116. Pettersson, P., Shen, Z., Johnsson, M. & Nygren, M. Thermal shock
resistance of α/β-Sialon ceramic composites. Journal of the European
Ceramic Society 21, 999-1005 (2001).
117. Pettersson, P., Shen, Z., Johnsson, M. & Nygren, M. Thermal shock
properties of sialon ceramics. Ceramic Materials and Components for
Engines, [International Symposium], 7th, Goslar, Germany, June 19-21,
2000, 147-152 (2001).
118. Lange, F. F. Powder processing science and technology for increased
reliability. Journal of the American Ceramic Society 72, 3-15 (1989).